Scanning Tunneling Microscopy Studies of Layered
Correlated Electron Systems:
Transition Metal Dichalcogenides and Iridates
B.S., University of Science and Technology of China, 2006
M.S., University of Colorado at Boulder, 2011
A thesis submitted to the
Faculty of the Graduate School of the
University of Colorado in partial fulfillment
of the requirements for the degree of
Doctor of Philosophy
Department of Physics
This thesis entitled:Scanning Tunneling Microscopy Studies of Layered Correlated Electron Systems:
Transition Metal Dichalcogenides and Iridateswritten by Jixia Dai
has been approved for the Department of Physics
Asst. Prof. Kyle McElroy
Prof. Daniel Dessau
The final copy of this thesis has been examined by the signatories, and we find that boththe content and the form meet acceptable presentation standards of scholarly work in the
above mentioned discipline.
Dai, Jixia (Ph.D., Physics)
Scanning Tunneling Microscopy Studies of Layered Correlated Electron Systems:
Transition Metal Dichalcogenides and Iridates
Thesis directed by Asst. Prof. Kyle McElroy
Strongly correlated electron problems, including high temperature superconductivity,
colossal magneto-resistivity, charge-density wave, heavy fermion phenomena, etc., have been
major research focuses in condensed matter physics for the past several decades. Involve-
ments of and competitions between different degrees of freedom and energy scales present
considerable difficulties for understanding these problems.
In this thesis, I have used home-built variable-temperature high resolution (spatial and
energy) spectroscopic imaging scanning tunneling microscopes (SI-STM) to study the to-
pography and the local single-particle tunneling spectroscopy in a family of two-dimensional
charge-density wave (2D-CDW) materials (TaSe2, TaS2, and NbSe2) and in a newly discov-
ered 5d Mott insulator Sr2IrO4 with strong spin-orbit coupling. In the 2D-CDW materials,
we have shown the strong lattice distortion and weak electron modulation accompanying
CDW transition, directly opposite to Peierls mechanism. We have also discovered that the
2D-CDW transitions in TaSe2 and TaS2 show involvement of the orbital degree of freedom,
shedding light on a long standing puzzle with their electrical resistivity anomalies. In the
novel 5d Mott insulator Sr2IrO4, we have found a large insulating gap of 620 meV, indicating
a stronger-than-expected correlation effect for a 5d electron system.
To my wife Ting Yan, our son Yian, my parents and my sister.
I firstly would like acknowledge my graduate advisor Prof. Kyle McElroy for his gen-
erous patience when teaching me about all kinds of experimental and theoretical details
and for treating me as an independent researcher from the beginning. His rigorousness in
experiments and analyses will affect and benefit me for life.
Thanks to Prof. Daniel Dessau for his great help with my experiments, for all of the
samples he shared with us, and for his encouragements during my hard times. Thanks to
Prof. Minhyea Lee for encouraging me to write my papers. Thanks to Prof. Michael Hermele
and Prof. Dmitry Reznik for sharing their thoughts on my papers. Thanks to Prof. Scott
Bunch for being nice and spending his precious time serving in my thesis committee. Thanks
to Prof. Chuck Rogers for allowing me to use many of his equipments.
I would also like to acknowledge our sample growers for providing us their high quality
single crystal samples, including Dr. Xiangde Zhu and Dr. Yuping Sun at High Magnetic
Field Laboratory (Hefei, China), Dr. Thomas Wolf at Karlsruher Institut fur Technologie
(Germany), Dr. Helmuth Berger at Ecole Polytechnique Federal de Lausanne (Switzerland),
and Prof. Gang Cao at University of Kentucky.
Thanks to my labmates Eduardo Calleja and Jacob Alldrege for helping me with my
experiments and my papers, and for discussing with me about many scientific and non-
scientific topics through out these many years. Thanks to Yue Cao for working closely with
me and for sharing his thoughts with me about research. Thanks to Xiaoqing Zhou for
reading my poorly written drafts and making suggestions on them. Thanks to Zhe Sun,
Qiang Wang, Jason Gray, Long He, Ted Reber, Nick Plumb, Justin Griffith and many many
others for their great encouragements and for helping out with my research.
Thanks to Tracy Buxkemper and Charlie Bowen in the Precision Instrument Shop.
My experiments are not possible without their precise and beautiful work. Thanks to Sid
Gustafson and Craig Joy in the Trades Teaching Lab for teaching me all of the details in the
Lastly and most importantly, I would like to acknowledge my parents for making all of
this possible. Thanks to my wife Ting Yan for understanding my pursuit in academia and
for supporting me in the past five years. As a husband, I owe her too much to be described
anywhere. Thanks to my son Yian, who always ‘reminds’ me of my responsibility and ‘urges’
me to work hard.
1 Introduction to Scanning Tunneling Microscopy and Spectroscopy 1
1.1 Tunneling phenomena . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1
1.2 Theory of Scanning Tunneling Microscope . . . . . . . . . . . . . . . . . . . 4
1.2.1 Constant current topographic imaging . . . . . . . . . . . . . . . . . 4
1.2.2 Spectroscopy measurement and imaging . . . . . . . . . . . . . . . . 6
1.3 Design of the UHV-STM . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7
1.3.1 Walker and scanner . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7
1.3.2 Tip and sample preparation . . . . . . . . . . . . . . . . . . . . . . . 12
1.3.3 Electronics: pre-amplifiers and STM controller . . . . . . . . . . . . . 14
1.3.4 Ultra-high Vacuum: chamber, load-lock and pumps . . . . . . . . . . 15
1.3.5 Cryostat . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 16
1.3.6 Vibration isolation . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17
1.3.7 Other experimental details . . . . . . . . . . . . . . . . . . . . . . . . 20
2 Charge-density wave in transition metal dichalcogenides 22
2.1 Introduction of charge-density wave . . . . . . . . . . . . . . . . . . . . . . . 22
2.1.1 Peierls mechanism and Fermi surface nesting . . . . . . . . . . . . . . 22
2.1.2 Mean-field approach . . . . . . . . . . . . . . . . . . . . . . . . . . . 24
2.1.3 LDOS with charge modulation . . . . . . . . . . . . . . . . . . . . . . 25
2.2 Charge-density waves in quasi-2D materials . . . . . . . . . . . . . . . . . . 28
2.2.1 Introduction to 2H-MX2 . . . . . . . . . . . . . . . . . . . . . . . . . 28
2.2.2 Recent progresses and remaining issues . . . . . . . . . . . . . . . . . 32
2.2.3 CDW gap opening . . . . . . . . . . . . . . . . . . . . . . . . . . . . 36
2.2.4 Doping and superconductivity . . . . . . . . . . . . . . . . . . . . . . 37
2.3 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38
3 Strong periodic lattice distortion in 2D charge-density wave systems 40
3.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 40
3.2 Previous STM study of topography in CDW systems . . . . . . . . . . . . . 42
3.3 Strong lattice distortion in 2H-MX2 . . . . . . . . . . . . . . . . . . . . . . . 43
3.4 Topographic images on CuxTaS2 . . . . . . . . . . . . . . . . . . . . . . . . . 52
3.5 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 54
4 Orbital-cooperative CDW transition in 2H-MX2 56
4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 56
4.2 Averaged LDOS on TaSe2 and TaS2 . . . . . . . . . . . . . . . . . . . . . . . 58
4.3 Spatially resolved LDOS study on TaSe2 and TaS2 . . . . . . . . . . . . . . . 61
4.4 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 65
5 Local density of states study of 5d Mott insulator Sr2IrO4 66
5.1 Introduction to Mott physics . . . . . . . . . . . . . . . . . . . . . . . . . . . 66
5.1.1 Mott insulator . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 66
5.1.2 Hubbard model . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 68
5.2 The novel Jeff=1/2 Mott insulator Sr2IrO4 . . . . . . . . . . . . . . . . . . . 68
5.2.1 Spatial extensions of d orbitals . . . . . . . . . . . . . . . . . . . . . 68
5.2.2 Spin-orbit coupling . . . . . . . . . . . . . . . . . . . . . . . . . . . . 69
5.2.3 Spin-orbit Mott insulators . . . . . . . . . . . . . . . . . . . . . . . . 70
5.3 Study of insulating gap in Sr2IrO4 with STS . . . . . . . . . . . . . . . . . . 72
5.4 Large insulating gap measured in Sr2Ir0.96Rh0.04O4 . . . . . . . . . . . . . . . 78
5.5 Study of impurity effects on insulating gap . . . . . . . . . . . . . . . . . . . 78
5.6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 82
A Vibration test of Room E2B37 83
B Pressure vs. time in a UHV pumpdown 85
C Feedback stability 89
2.1 CDW and superconductivity transition temperatures of 2H-MX2 . . . . . . . 35
1.1 Quantum tunneling of electrons. . . . . . . . . . . . . . . . . . . . . . . . . . 1
1.2 Tunneling current as integration of density of states . . . . . . . . . . . . . . 2
1.3 Schematic diagram of a Scanning Tunneling Microscope . . . . . . . . . . . . 5
1.4 An overview of the UHV-STM system . . . . . . . . . . . . . . . . . . . . . 8
1.5 Solidworks drawing of the STM scan head . . . . . . . . . . . . . . . . . . . 9
1.6 Walker piezo stack . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10
1.7 Tubular piezo scanner . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11
1.8 Images of tip and the etching process . . . . . . . . . . . . . . . . . . . . . . 12
1.9 Images of sample holder . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13
1.10 Modeling the noise of the pre-amplifier . . . . . . . . . . . . . . . . . . . . . 14
1.11 Single-stage vibration isolation modeling . . . . . . . . . . . . . . . . . . . . 18
1.12 Transfer function of a single-stage isolation system . . . . . . . . . . . . . . . 19
1.13 Diagram for thermal sink with electrical isolation . . . . . . . . . . . . . . . 20
2.1 Lindhard response function for free electron systems . . . . . . . . . . . . . . 23
2.2 Ideal Peierls transition for a 1D metallic system . . . . . . . . . . . . . . . . 24
2.3 LDOS evolution with the periodicity of CDW from mean-field theory calculation. 26
2.4 Representative LDOS spectra in an electron-driven CDW. . . . . . . . . . . 27
2.5 Topography and crystal structure of the 2H-NbSe2 . . . . . . . . . . . . . . . 29
2.6 Topography of the 2H-TaS2 (a) and TaSe2 (b). . . . . . . . . . . . . . . . . . 30
2.7 Two CDW transitions in TaSe2 . . . . . . . . . . . . . . . . . . . . . . . . . 31
2.8 Possible fermi surface nesting in 2H-TaSe22 . . . . . . . . . . . . . . . . . . . 32
2.9 Phonon anomaly in 2H-NbSe22 . . . . . . . . . . . . . . . . . . . . . . . . . 33
2.10 Conductivity enhancement with CDW transitions in 2H-MX2 . . . . . . . . . 34
2.11 Local density of states measurement in NbSe2. . . . . . . . . . . . . . . . . . 36
2.12 Phase diagrams of Cu intercalation into TiSe2 and TaS2 (Cu2TiSe2 and CuxTaS2) 37
3.1 Previous STM images of Ge(111) surface covered by 1/3 monolayer of Sn. . . 42
3.2 Previous STM images of NbSe3 . . . . . . . . . . . . . . . . . . . . . . . . . 43
3.3 Topographic image of 2H-TaS2 including a CDW mismatch. . . . . . . . . . 45
3.4 Topographic images showing symmetrization and antisymmetrization on 2H-
TaS2 at 52 K. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 47
3.5 Topographic images of NbSe2 and TaSe2 at 5 K. . . . . . . . . . . . . . . . . 49
3.6 Topographic images on 2H-NbSe2 at T = 6 K. . . . . . . . . . . . . . . . . . 51
3.7 Topographic images with various bias voltages on CuxTaS2 (x = 0.04). . . . 53
4.1 Band structure of TaSe2 from first principle calculation. . . . . . . . . . . . . 57
4.2 LDOS measurements on TaSe2 and TaS2 . . . . . . . . . . . . . . . . . . . . 59
4.3 High voltage LDOS on TaSe2 . . . . . . . . . . . . . . . . . . . . . . . . . . 60
4.4 Ratio map of TaSe2 and intra-unit-cell variation . . . . . . . . . . . . . . . . 62
4.5 Local distortion and related shifts in orbital energies. . . . . . . . . . . . . . 63
4.6 Ratio map and intra-unit-cell variation of LDOS . . . . . . . . . . . . . . . . 64
4.7 Ratio map at 100 mV showing the asymmetry is intrinsic. . . . . . . . . . . 65
5.1 Density of states change in Mott transition . . . . . . . . . . . . . . . . . . . 67
5.2 Spatial extensions of d orbitals . . . . . . . . . . . . . . . . . . . . . . . . . . 69
5.3 Splitting of 5d levels in Sr2IrO4 . . . . . . . . . . . . . . . . . . . . . . . . . 71
5.4 Topography and atomic structure of Sr2IrO4. . . . . . . . . . . . . . . . . . . 73
5.5 The 620 meV intrinsic energy gap in Sr2IrO4. . . . . . . . . . . . . . . . . . 75
5.6 Bias dependent topography in Sr2IrO4. . . . . . . . . . . . . . . . . . . . . . 77
5.7 Large insulating gap measured on Sr2Ir0.96Rh0.04O4. . . . . . . . . . . . . . . 79
5.8 Tip induced band bending in Sr2IrO4. . . . . . . . . . . . . . . . . . . . . . . 81
A.1 Vibrational test of Room E2B37 . . . . . . . . . . . . . . . . . . . . . . . . . 83
B.1 Plot of pressure versus time of the UHV-STM system. . . . . . . . . . . . . . 86
B.2 Plot of pressure versus time of the UHV-STM system during normal operation. 87
C.1 STM feedback loop . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 89
C.2 Transient response of the tip . . . . . . . . . . . . . . . . . . . . . . . . . . . 90
Introduction to Scanning Tunneling Microscopy and Spectroscopy
1.1 Tunneling phenomena
Quantum tunneling, a classically forbidden process of electrons (particles) penetrating
through energy barriers, was experimentally verified by Leo Esaki in semiconductors  and
by Ivar Giaever in superconductors  respectively. Their work of single particle tunneling
led towards the prediction of Cooper pair tunneling (Josephson effect) by Brian D. Josephson
. This same process is also the essence of nuclear alpha decay, as initially pointed out by
George Gamow , where the microscopic particle that tunnels is the alpha particle.
Figure 1.1: Quantum tunneling of electrons between two metals separated by a vacuum gap.
Tunneling is made possible by the fact that in quantum mechanics particles are de-
scribed by wave functions that are extended in space. A simplified picture of tunneling in
one dimension is shown in Fig. 1.1. When the two metals are brought close to each other
(3 − 10 A for STM junctions and a few nm or more for planar junctions), the exponential
tails of wave functions overlap before point contact takes place. In the low energy limit
(kinetic energy much smaller than barrier height), the electron wave functions between the
two metals are linked via an exponential decaying term,
|ψ2|2 = e−2κz |ψ1|2 , (1.1)
where ψ1 and ψ2 denote the electron wave function on the two sides. The characteristic decay
length of the wave function is κ =√2mφ~
φ(eV )A−1, m is the mass of electron and
φ is the height of the vacuum barrier, which is approximately the (averaged) work function
of the metals. Since work functions for most materials are in the range of 4 − 6 eV, much
larger than the electron kinetic energy, it is a good approximation to treat the two sides of
the junction with the same work function (∼5 eV). This approximation of work function
values results in a roughly unchange decay constant, κ ≃ 1 A−1. In terms of electron density
(magnitude square of wave function), the exponential decay is around e2 ≃ 7.4 times per
A: the tunneling current will decrease 7.4 times when the distance between two metals is
increased by 1 A.
Figure 1.2: Tunneling current as integration of density of states. The tunneling process isonly possible between occupied states on one side to the unoccupied states of the other side.The difference of the Fermi levels is set by the bias voltage.
When the two sides of the junction are connected with no voltage (equal Fermi levels
EF), the electrons can hop back and forth due to thermal activation around EF, but there is
no net current. However, when a voltage V is applied between the two sides, a net current
can be induced. The current can be calculated using the Fermi’s golden rule ,
−∞[f(EF − eV + ǫ)− f(EF + ǫ)] ρs(EF − eV + ǫ)ρt(EF + ǫ)|M |2dǫ, (1.2)
where the f(E) is the Fermi-Dirac distribution function, and ρs and ρt are the density of
states (DOS) of the two sides. This equation is visualized in Fig. 1.2.
In Fig. 1.2, we have drawn a relatively featureless DOS on the right side of the junction,
which is a normal scenario for the study in this thesis, since we usually prepare our probe
tips such that there is no structure in its DOS. Furthermore, we can simplify Eqn. (1.2) by
assuming that temperature is low comparing to energy scale of interest and the tunneling
matrix element M is energy independent (following Bardeen ), M ∼ e−κz. With these
approximations, we can reduce Eqn. (1.2) as,
ρs(EF − eV + ǫ)dǫ, (1.3)
from which we can see that,
dV∝ ρs(EF − eV ). (1.4)
The differential conductance measurement is simply proportional to the density of states.
In this thesis, I will refer to local density of states (LDOS) as dI/dV measurement, but
one should always be aware that they are only equal to each other with the approximations
mentioned above, at best.
The density of states in superconducting lead, as measured by Giaever , provided
strong evidence for the BCS theory of superconductivity and triggered a lot of interests in
studying electronic structures with tunneling experiments. However, since planar junctions
are only able to measure DOS on average, it became highly desirable to take advantage of
the same effect and measure local density of states. In 1982, it was finally possible because
of the invention of Scanning Tunneling Microscope by Binnig and Rohrer .
1.2 Theory of Scanning Tunneling Microscope
A Scanning Tunneling Microscope (STM) takes advantage of the electron tunneling
effect between an atomically sharp tip and the sample under investigation. It usually consists
of four basic units: coarse motion actuator, fine motion actuator, current amplifier, and
electronic control unit. As shown in Fig. 1.3, during the operation of a STM, a bias voltage
is firstly applied to the sample and then the metallic tip is brought close to the surface of the
sample by the coarse motion actuator, and then feedback is turned on immediately when a
tunneling current is detected by the control unit. The tiny current (∼ pA−nA) is detected
by a transimpedance amplifier with gain at 0.1 − 10 GΩ, which converts this small tunneling
current signal to a voltage.
1.2.1 Constant current topographic imaging
Due to the high sensitivity of tunneling dependence on the distance between tip and
sample, it is usually beneficial to operate the STM in constant current mode, in which the
tunneling current is maintained constant by a feedback mechanism. In the constant current
mode, the STM controller takes the voltage signal from the current amplifier, compares it
with the pre-set value and adds the difference to the output z-piezo voltage with a gain.
This forms a feedback loop involving the z-piezo, tunnel junction, current amplifier, and
the control unit, and assures that the tunneling current is constant. More details about the
feedback system can be found in Appendix C.
While the feedback loop is active, scanning voltages can be applied on x and y-piezo
to move the tip line by line across the sample surface. Since the z-piezo is controlled by the
feedback loop so it closely follows the height profile of the surface, namely the topography.
Recording the height profile with the x and y information, one would end up with a 2D
image of the surface height under the constant tunneling current condition, namely constant
Figure 1.3: Schematic diagram of a Scanning Tunneling Microscope. The STM controlleroutputs a bias voltage Vbias, five high voltage signals for controlling the tube scanner (z, +x,−x, +y, −y), and other voltages if necessary. A sharp metallic tip is firmly attached to thetube scanner. When the tip is a few A away from the surface and the sample voltage Vbiasis nonzero, a tunneling current will be induced between the virtually grounded tip and thesample. This current is converted to voltage signal by a transimpedance amplifier, and sentover to the STM controller. The controller then compares the tunneling current with theset point value (set by user), and adds the error to the z-piezo voltage output with a gain(set by user). This feedback loop is the essence of the constant current mode. While thefeedback loop is active, voltages can be sent to x/y scanner to scan the tip across the sampleand the tip height information during a scan is essentially a constant current topographicimage. A lock-in amplifier is used to perform spectroscopic measurements.
Since the tunneling process is only sensitive to electrons/holes with energy between EF
and EF + eVbias and feedback loop further constrains the tunneling current to be constant,
I(x, y) = I0e−z/z0
LDOS(x, y, ǫ)dǫ = const., (1.5)
constant current imaging essentially reflects the integrated local density of states and mor-
phology of the surface through z,
z(x, y) = −z0 ln(
+ z0 ln
LDOS(x, y, ǫ)dǫ
where z0 is converted from the κ in Eqn. (1.1), z0 =12κ.
1.2.2 Spectroscopy measurement and imaging
Besides the constant current imaging mode, STM is also often operated in the spec-
troscopy mode. In this mode, the xy scanning and the feedback loop is temporarily disabled
(constant height), and the bias voltage is swept from one value to another one, while the
tunneling current (I−V curve) is recorded. More often, dI/dV is measured at the same time
with a lock-in amplifier by adding an AC voltage with small amplitude (∼ 1− 10 mVrms) to
the bias voltage and measuring the signal in tunneling current with the same frequency as
the added signal. From the Taylor expansion of the tunneling current,
I(V0 + Vm cos(ωt)) = I(V0) +dI
Vm cos(ωt) + ..., (1.7)
we can see that the lock-in amplifier actually measures this quantity,
dV· Vm ·R · 10V
where Vm is the rms of the ac modulation, R is the gain of the preamplifier, and sens is the
sensitivity of the lock-in amplifier, usually set to 50 − 200 mV . If the lock-in amplifier is
set to output ‘Display’ instead of ‘X’ or ‘Y’, the last term should be dropped, but the signal
noise ratio coming out of the lock-in will be affected due to the signal reduction from V to
Furthermore, for deliberately designed systems with long continuous operating time,
like the ones in our lab, it is possible to run with the spectroscopic imaging mode. In this
mode, dI/dV measurement is performed on every point of a pixel grid. The feedback loop is
activated when scanning the tip in between points and deactivated when taking the dI/dV
measurement. This process is usually called as ‘spectroscopic imaging’, ‘dI/dV mapping’ or
simply ‘mapping’. With our UHV-STM, a 128 × 128 points dI/dV map with 256 energy
points takes about 16 hours.
1.3 Design of the UHV-STM
Our UHV-STM system includes a cryostat purchased from CreaTec, a STM chamber
customized with A&N corp, a load-lock with a turbo-molecular pump, an Ion/TSP pump
from Varian Inc. and a home-made STM scan-head.
1.3.1 Walker and scanner
A coarse motion actuator is needed for bringing the sharp tip to a small distance
(usually ∼ 100 nm) away from the sample. There are more than a few types of coarse
approach mechanisms, including the walker , the beetle , etc. In our UHV-STM, a
Pan-style walker design was adopted. Each leg of the walker is consisted of four sheets of
piezo stacked together with alternating polarization directions, as shown in Fig. 1.6. The
size of each piezo sheet is 0.20” × 0.20” × 0.020”.
The shear-mode piezo operates in the manner shown in Fig. 1.6a. When an electric
field E perpendicular to the polarization P is applied to the piezo pad, the corresponding
motion of the piezo pad is to shear between the top and bottom surfaces. The equation that
describes this motion is as follows,
∆x = d15Eyh = d15Vy, (1.9)
where ∆x is the amount of shear motion. This ∆x is often not directly proportional to
(d) Inner cryogen bath
Figure 1.4: An overview of the UHV-STM system. (a) Image of the entire system. From topto bottom are: cryogen and gas ports, electric feedthroughs, body of the dewar, STM cham-ber and the table attached on top of 4 air springs, the ion pump and titanium sublimationpump. On the backside, we can see part of the loadlock and turbo pump system. On top ofthe table is a Model 1212 current preamplifier (DL instruments), which is usually replacedby our home-made pre-amplifier. (b) Image taken through the viewport. From inner out,we see the body of the STM, the inner, the outer cryo-shield and the UHV chamber with aviewport. (c) Image of the STM and cryo-shields when it is detached from its chamber. (d)Image of the STM suspended by the springs. The bottom copper piece is for Eddy currentdamping.
Figure 1.5: A solidworks drawing of the STM scan head. The top and bottom ‘gray’ piecesare made out of titanium, while the center ‘blue’ body is macor. The numbers indicate theimportant small parts, including (1) sample holder, (2) piezo scan tube and tip assembly,(3) sapphire prism, (4) one of the six walker piezo stacks, and (5) the scan tube holder, towhich (2) is glued.
the single-step size of the walker, since the walker is also sensitive to other conditions like
surface cleanness and the tension exerted by the BeCu spring (the front cover in Fig. 1.5).
The walking step size of the UHV-STM is ∼ 200 - 300 nm at room temperature and ∼ 40 -
60 nm at helium temperature with the driving voltage set to 320 V.
Side view 3D view
Figure 1.6: Operation of shear mode piezo (top). Walker piezo stack with side view (left)and 3D view (right). The piezo sheets are glued together with copper foils by conductingepoxy (H21D) and the copper tabs sticking out of the stack are electrical contacts.
The mostly used fine motion actuator is the tubular scanner invented by Binnig and
Smith . Shown in Fig. 1.7 is a schematic diagram of such a tubular scanner and how
the electrodes are connected. The dimension of the scanner in our UHV-STM is as follows,
L = 0.25”, OD = 0.125” and ID = 0.080”. When voltage is applied to electrode z, the
scanner will extend or shrink along its length direction. The total z-range of the scanner at
77 K is about ±180 nm with ±420 V on the z voltage. When voltage is applied to the xy
electrodes, the scanner will tilt in the corresponding directions. For instance, when voltage
is applied to ±x, the scanner tilt in the x direction. The detailed equations describing the
motion of the scanner are as follow,
∆x =2√2d31V L
πDh, ∆z = d31V
where the voltages applied on ± quadrants (of x or y) are assumed to be with the same
magnitude but opposite signs.
y Top view
Figure 1.7: A diagram for the tubular piezo scanner. The piezo is polarized in the radialdirection and coated with layers of metal (usually Au or Ni) on both inner and outer surfacesof the tube. The outer conductor is further split into four quadrants, ±x and ±y, along thelength direction. Applying pos. (neg.) voltage on z will extend (shorten) the scan tube inthe length direction. Applying voltage on x/y quadrants (opposite sign on ± quadrants) willbend the scan tube in x/y directions.
All of the piezos, including shear-mode pads and tubular scanner, are of type PZT8,
purchased from companies including EBL Products, Inc. and Boston Piezo Optics, Inc.
PZT8 is chosen for its high temperature stability and low mechanical hysteresis (creep-
ing). The important parameters of PZT8 for our applications are the piezoelectric constants
d15 = 330 pm/V and d31 = −95 pm/V . The piezo constants of PZT8 changes slowly with
temperature. The relative ratio of the piezo constants at 4 K, 77 K and room temperature
is roughly, 2/3:1:2. This ratio comes from calibration using the XY piezo calibrations, so it
depends on the tip length and has an error bar as high as 10% or more.
1.3.2 Tip and sample preparation
Figure 1.8: Images of tip and the etching process. (a) Image of the tip etching process. Thecenter wire is a tungsten wire with 0.25 mm diameter and the outer ring is made out ofstainless steel. A positive dc voltage (2 ∼ 6 V) is applied on the tungsten wire. (b) Imageof an etched tungsten tip taken under a microscope with 100 × magnification. (c) Imageof the tip while in the tip holder and ready for performing experiment. The tungsten tip isbent to a zigzag shape in order to offset the tunneling location from the rotational center by∼ 1.5 mm.
We use electrochemically etched tungsten tips in our tunneling experiments. During an
etching process, a tungsten wire of diameter 0.25 mm is pulled through a film of 2M NaOH-
water solution, and then a voltage is applied between the tungsten wire and the stainless
steel ring (Fig. 1.8). The film is formed by dipping the stainless steel ring into the NaOH
solution. The applied voltage is usually set to 2 to 6 Volts. Different etching voltages usually
result in different etching rates. The etching rate can be estimated via the rate of bubble
formation around the stainless steel ring. Occasionally, the film bursts during the etching
process, which requires reforming the film and restarting the etching process. This can result
in different shapes of the tip apex, observable under optical microscopes.
Freshly etched tip needs to be cleaned by DI water and alcohol, and then checked under
a microscope with magnification 100 × or above. This process can assure the apex of the tip
is less than a few micron or under the diffraction limit, which is sufficient for our experiments
since field emission usually results in blunt tip apex with radius close to µm. Atomically sharp
tips usually require further preparation after field emission. A commonly used method is to
mechanically collide the tip with a gold surface and retract before re-engaging to tunneling.
Further scanning on clean gold surface with high tunneling current (e.g. 1 nA) and high bias
voltage (e.g. 1 V) can stabilize the tip. However, mostly importantly, the density of states
of the tip should be relatively featureless before it can be used to investigate a sample. This
is possible since the density of states on amorphous gold sample is flat for reference.
Figure 1.9: Images of a sample and the sample holder. (a) An image of the sample holderused in the UHV-STM, glued with a piece of gold and a Bi-2212 sample. (b)Image of thecleaved surface of Bi-2212.
Cleavable samples are usually attached to the sample holder with conducting epoxy
(H21D). After the glue cured, a short rod is then attached directly on top of the sample. This
short rod is knocked off to cleave the sample and yield a fresh surface, after the sample is
introduced into vacuum. In our UHV-STM, this is realized by positioning the sample transfer
manipulator so that the sample cleave rod sits at the position of the LN2 shield door and
then the shield door is dropped to hit the cleave rod. The sample with the fresh surface is
then inserted into our STM and the entire scan-head reaches temperature equilibrium a few
Together with the sample, we can also glue a piece of press-flattened gold, as the target
for field-emission tip preparation. With the two targets symmetrically attached around the
rotational center and the tip bent carefully, we can easily switch between tunneling with
either gold or another sample. With this method, we can reduce the sample exchange time
from 4−5 hours down to about 1 hour. It also greatly improves the experimental success
rate on rare samples, as long as the cleave is successful.
1.3.3 Electronics: pre-amplifiers and STM controller
In order to measure the tunneling current, a type of pre-amplifier called transimpedance
amplifier is needed. This type of amplifier converts the tunneling current signal into voltage,
so they are also called IVCs (I-V converters). We usually use two transimpedance pre-
amplifiers: the first one is the Model 1212 from DL electronics and the second one is home-
built with OPA627 or OPA140.
The amplification of a transimpedance amplifier is controlled by a feedback resistor
which in our application is on the order of GΩ. The value of this resistor is also the gain of
this amplifier, V = I × R where I is the input and V is the output. In order to get a clean
Figure 1.10: Modeling the noise of the pre-amplifier.
tunneling signal, electronic noise of the amplifier needs to be considered. Shown in Fig. 1.10
is a minimum model for analyzing this electronic noise. The current source i is the tunneling
current in the STM junction, in and vn are the current and voltage noises of the op-amp
(OPA627 or OPA140) itself, and the voltage noise ven is the thermal noise of the feedback
resistor, ven =√4kBTRf . Another very important parameter that limits the frequency at
which the spectroscopy work can be performed is the shunt capacitance between the tip wire
and the ground, CS. Combining all of these noises, we get
v2n + i2n +4kBT
Here, the units of currents and voltages are A/√Hz and V/
√Hz. This equation can be
used as an ultimate limit for electronic noise. However, most of the time larger noise comes
from external sources like crosstalk and grounding loops, for which more detailed diagnoses
will be needed.
In order to move the STM tip in the xyz directions, high voltages need to be applied on
the inner and outer electrodes of the scanner (Fig. 1.7). These voltages are provided by the
STM controller (MFP-3D from Asylum Research), which is able to provide 3 pairs of high
voltages (six channels in total) up to ±420 V with resolution of 24 bits. This bit resolution,
when converted into real space xyz resolution of the scanner, is roughly δz = 0.022 pm and
δx = 0.381 pm at T = 77 K.
1.3.4 Ultra-high Vacuum: chamber, load-lock and pumps
STM experiment generally requires ultra-high vacuum (< 10−9 torr) environment due
to the high sensitivity of the vacuum junction to external objects like gas molecules, and the
strong electric field within (∼ 109 V/m) makes the situation worse. The existence of ‘free’
gas molecules can cause noise spikes in the tunnel current and make the junction unstable.
To achieve such a high vacuum environment, a great deal of effort is required, especially
for STM experiment at temperature higher than ∼ 10 K, where cryogenic vacuum is not
In our UHV-STM, a 70 l/s turbo pump (with a Xtr-dry 250 backing pump) is used
to evacuate the chamber from ambient pressure down to the 10−7 torr range, before an ion
pump and the heater for bakeout are turned on.
Due to fact that most materials will absorb water or air molecules on their surfaces and
they will outgas when pressure is reduced, particular care is needed for choice of materials for
UHV experiments. Most metals, including stainless steel, iron, nickel, copper, aluminum,
titanium, even tin and lead, are fine for vacuum, but materials with high vapor pressure
(room temperature or during bake-out), like zinc and cadmium, should definitely be avoided.
This excludes a very commonly used material, brass. Stainless steel, aluminum, and copper
are widely used in our experiments. Aluminum bronze (Al-Cu alloy) is used for our sample
holders, due to its high strength and machinability. Plastics are usually bad for vacuum
since they trap gas molecules deeply into the bulk and have low ‘melting’ points. In our
UHV systems, there are only three types of plastics that have been used, including PEEK,
kapton (polyimide) and teflon. Following this same reasoning, most of the glues are not
suitable for UHV and the two types we used are Torr-Seal high vacuum epoxy and H21D
silver conducting epoxy. A relatively complete reference for UHV compatible material choice
is Ref. .
To achieve UHV condition, we need to firstly bake-out the chamber which basically
expedites the out-gassing from the chamber walls by heating up the entire system to 120
to 140 C. A bake-out is very effective for removing water molecules from the UHV system,
which is the biggest limiting factor of vacuum in the range of 10−4 to 10−9 torr. A normal
pumpdown of the UHV-STM system can be found in Appendix B.
The UHV-STM cryostat, purchased from Createc, is consisted of two cryogen baths,
including a 14 liters of LN2 bath and a 4 liters of LHe/LN2 bath. With the heat load from
wires in the current configuration, the outer bath can last for ∼ 72h and the inner bath can
last for 36 hours with LHe or more than 20 days with LN2.
The inner dewar can also be pumped to low pressure (e.g. 1 torr) to lower the cryogen
boiling point. The pumping is carried out by simply connecting a rotary pump to the outlet
of the inner dewar with a long hose (> 30 feet). In order to reduce the vibration from the
pump, we place the pump out of the STM room and press the hose firmly by lead bricks in 2
- 3 positions. With LN2 in the inner dewar, we can pump it so that the base temperature is
lowered to 50 K instead of 77 K. At such a low temperature nitrogen is solid and the cooling
power thereafter comes from the sublimation of solid nitrogen.
1.3.6 Vibration isolation
Mechanical vibration from the environment is ubiquitous, and a lot of experimental
equipments like vacuum pumps, cryogenic dewars, electronic boxes have their own vibration
that cannot be eliminated. For a scanning tunneling microscope, the crucial vibration is
the relative motion between the tip and the sample. When the feedback loop is turned off,
relative vibration as small as 1 pm could be seen in the tunneling current. In order to reduce
this relative motion, there are several steps in general that need to be done. The first one is
to build a compact and rigid scan head so that the acoustic path between the tip and sample
is short and stiff. The walker  is a good example of rigid design with a high resonance
frequency. The second important thing to do is to remove as much of the vibrational sources
(vacuum pumps, electronic boxes, human beings, etc.) from the vicinity of the experiment.
The third to do is to isolate the environmental vibration from the STM (air springs, acoustic
isolation room, etc.).
In our UHV-STM system, we have placed the experiment in an acoustically isolated
room (sound room), with most of the electronic boxes outside. We also turn off the turbo
pump on the load-lock during tunneling experiments. Furthermore, we have used an air
spring system, and two spring-damping stages (Fig. 1.4). The air springs separate the UHV
chamber from the floor, while the two spring-dampening systems isolate the scan-head from
the UHV chamber at two different levels. In our first spring-damping system, the spring is
actually a soft tube to which the inner cryogen bath is attached, and the damping is provided
by a copper disk moving within a magnetic field (Fig. 1.4), known as Eddy current damping.
The second spring-damping system is composed of four stainless steel springs with which the
scan head is suspended and a copper cross sitting inside magnetic field provided by SmCo5
permanent magnets on the bottom of the inner cryo-shield.
Figure 1.11: Single-stage vibration isolation modeling.
Here we describe the mechanism of a spring-damping isolation system with a simple
model. Suppose there is a spring-mass system attached to a wall (see Fig. 1.11). The mass
could be viewed as our experiment and the wall is the environment, which is moving by itself
y = y(t). Our objective is to relate the motion of the mass x = x(t) to y(t). The equation
of motion is simply,
mx+ γ(x− y) + k(x− y) = 0, (1.12)
where k is the spring constant and γ is the dampening term. Solving this equation with trial
solution x(t) = x0e−iωt and y(t) = y0e
=iγω + k
−mω2 + iγω + k, (1.13)
The magnitude of this ratio is defined as the transfer function,
k2 + γ2ω2
(k −mω2)2 + γ2ω2=
1 + β2ω2/ω20
Here β is the reduced damping factor β = γω0/k and ω0 is the resonance frequency of the
spring-mass system ω0 =√
Two extreme cases for the Eqn. 1.14 and the resonance amplitude could be easily
extracted and could also be seen in Fig. 1.12. At zero frequency, the transfer function is
simply one. At high frequency, T0(ω) = βω0/ω which means the lower β is the better
the isolation at high frequency will be. At the resonance frequency ω = ω0, T0 =√
which indicates that small β will cause sharp resonance and therefore should be avoided.
To balance the resonance at ω0 and isolation at high frequency an ideal condition could be
roughly β = 1. In our UHV-STM adjusting β is realized the via changing the Eddy current
damping. For example the thickness of the copper piece and the strength of the permanent
magnets both could be varied to increase to decrease the damping factor β. However, since
the conductivity of copper changes with temperature, it is quite hard to meet the ideal
requirement at all temperatures.
0.12 4 6 8
12 4 6 8
102 4 6 8
β = 0.1
β = 0.2
β = 0.5
β = 1
β = 2
Figure 1.12: Transfer function of a single-stage vibration isolation system.
After all, the above discussions are all based on ideal situations, while in reality vibra-
tional shorts (e.g. wires that connect the cryogen bath and the STM scan-head) are also
very crucial for vibrational noise performance. Checking for these shorts will be absolutely
necessary to minimize the vibrational noise for tunneling experiments.
1.3.7 Other experimental details
For a STM experiment at high temperature (e.g. 77 K) the differential thermal expan-
sion between different parts of the STM scan-head will cause significant amount of thermal
drift between the tip and sample due to both experiment-related operations and temperature
fluctuation caused by weather or ambient pressure changes. Thermal stabilization on the
scan-head thus becomes necessary. In our UHV-STM we have used an home-made resistive
heater and a Lakeshore temperature controller to stabilize the STM temperature within a
few mili-Kelvin of the set temperature. At the meantime, we have thermally sunk the STM
with the cryogen bath with a copper braid. The size of the copper braid can be adjusted to
balance in between the base temperature, the cooling rate, and the boil-off rate.
Figure 1.13: Diagram for making thermal sink with electrical isolation for the top-plate ofSTM scan-head. The sample bias voltage could be as high as 300 V during field emission.For good thermal sinking the size of the sapphire could be as large as 0.5 by 0.5 inch andthe thickness of it could be as small as 0.02 inch. If sapphire is not available, quartz couldalso be used instead. Since PEEK is not a strong material, tightening of these screws shouldbe very gentle, usually less than finger strength, but the performance of this thermal sink atlow temperature is still quite good.
While thermally connecting the entire STM scan-head is necessary for the low-drift
requirement, it is also necessary to electrically isolate some parts. For example, the top-
plate of the scan-head where sample bias voltage is attached needs to be separate from all
of the other components including the cryogen bath, the aluminum shields, the heater coil
and the temperature sensor. These isolations were done with PEEK screws/rings, sapphire
pieces, and Kapton wire insulations. It is also necessary to connect the bottom-plate of the
scan-head with the top-plate in order to reduce the thermal equilibrium time within the
STM scan-head. This is done by separating the aluminum piece that connects the top and
bottom plates from the top-plate by a piece of sapphire and clamped together with PEEK
screws. The electrical isolation between the top-plate and the cryogen bath was done in a
similar fashion at the interface between the copper braid and the cryogen bath. A simplified
diagram of this type of thermal sinking and electrical isolation could be seen in Fig. 1.13.
In order to reduce the heat load on the STM and the cryogen baths we have used only
manganin and stainless steel wires (mostly AWG 36 from MWS Wire Industries) connecting
the top feedthroughs (Fig. 1.4) and the STM scan-head. Additional teflon heat-shrink tube
were used to protect the manganin/SS wire braids against sharp parts of the vacuum cham-
ber. The tip-line carrying the tunneling current of order pA to nA is a semi-rigid coaxial
cable (SC-119 from Coax Co., LTD.). This coax cable uses stainless steel for both inner
and outer conductors and polyimide for isolation. To avoid shorting the vibration isolation
for the STM, semi-rigid cable was not used at the last section when connecting to the STM
scan-head. This part is replaced with a coax cable (Type CC-SC-500 from Lakeshore).
Charge-density wave in transition metal dichalcogenides
2.1 Introduction of charge-density wave
Charge-density wave breaks the lattice translational symmetry of a crystal by redis-
tributing the electron density in a spatially periodic manner. It occurs in a wide range of
materials, including both quasi-1D and quasi-2D systems. For quasi-1D systems , it has
been found in NbSe3 (and many siblings of it), (Ta2Se4)I, blue/purple bronzes, many 1D
organic conductors, 1D metallic chains on Si surface , etc. For quasi-2D CDW systems,
the research has been mainly focused on the layered transition metal dichalcogenides (TMD
or MX2), Pb/Sn covered Ge(111) surface, etc. The rare-earth tritellurides, RTe3 (R = rare-
earth element), are a class of materials that are quasi-two-dimensional in structure but the
CDW in them is unidirectional [14, 15]. Review papers could be found in Ref. [12, 16, 17]
for 1D systems and in Ref.  for 2D TMDs.
2.1.1 Peierls mechanism and Fermi surface nesting
We will start by introducing the Peierls mechanism in a simple 1D metal. For an atomic
chain with partially filled band (e.g. one electron per site), the response of the system to
external electric field is described by the Lindhard function,
(2π)dfk − fk+q
ǫk − ǫk+q
where ǫk is the energy band (energy-momentum dispersion relation of electrons) and fk =
f(ǫk) is the Fermi-Dirac distribution function, f(ǫ) = 1e(ǫ−µ)/kBT+1
. Results of calculation for
free-electron systems with different dimensionalities could be found in Fig. 2.1. One would
immediately notice that for the 1D system, the Lindhard response function is diverging at
2kF, which is not surprising since for a 1D system all parts of the Fermi surface (basically
two points) are connected by the same wave vector to other parts of the Fermi surface.
Similar divergence is possible for 2D systems too, since anisotropic 2D systems can have
large sections of Fermi surface that are parallel to each other. This is the basic idea of
‘Fermi surface nesting’. Mathematically checking the nesting properties of a particular Fermi
surface is possible by simply doing the auto-correlation of the spectral intensity map at the
Fermi level (also called as the Fermi surface). If nesting condition is satisfied, it would show
up as peak(s) in the auto-correlation map.
Figure 2.1: Lindhard response functions for free-electron systems in different dimensions.These are qualitative sketches following Ref. .
As a result of the divergence in χ(q), the system undergoes a structural phase transition;
i.e., the system enters into another lower energy state, the CDW state. In this new state,
the electron density is redistributed according to the wave vector 2kF and the ions are
displaced due to electron phonon interaction (periodic lattice distortion). However, since
lattice distortion increases the elastic energy, it is only a second order effect.
Figure 2.2: Ideal Peierls transition in a 1D metallic system. A gap is opened at EF (a-b),and the density of electron forms a wave in real space (c-d).
The concept of CDW, in its more general form of “charge ordering”, is widely used
in other correlated electron systems like cuprate and iron-based high-Tc superconductors
[19, 20]. It also has been suggested that the checkerboard in BSCCO is intimately tied with
a CDW .
2.1.2 Mean-field approach
This part is a summary of the important results in Ch.3 of the book by Gruner .
To describe the charge density wave formation, we start by introducing the Frohlich
Hamiltonian including both electronic and phononic contributions,
bq + b†−q
where ak (bq) and a†k (b†q) are electron (phonon) annihilation and creation operators.
After the CDW order sets in, the phonon mode at 2kF becomes macroscopically occu-
pied. The average occupation on this mode is the order parameter of the CDW transition,
|∆|eiφ = g(
The renormalized phonon frequency (the phonon frequency that can be measured ex-
ω2ren,q = ω2
~χ(q, T ), (2.4)
from which we can see the softening of phonon (since χ<0). In the mean field approximation,
the Frohlich Hamiltonian is simplified as,
ǫka†kak + 2g
〉+ a†k−2kFak〈b−2kF 〉
+ 2~ω2kF 〈b2kF 〉2, (2.5)
This quadratic Hamiltonian can be diagonalized using a Bogoliubov transformation,
γ1,k = Uke−iφ/2a1,k − Vke
iφ/2a2,k, γ2,k = Vke−iφ/2a1,k + Vke
with the diagonalizing condition being,
2ǫkUkVk + |∆|(
U2k − V 2
= 0, U2k + V 2
k = 1, (2.7)
which yield the following solutions,
V 2k =
, U2k =
As a result, the band dispersion is BCS-like,
Ek = sign(k − kF )(
, ǫk = ~vF (k − kF ), (2.9)
and the ground state wave function is given as,
|0〉 , (2.10)
2.1.3 LDOS with charge modulation
In a CDW state, the electronic density is modulated with the wave length 2π/2kF.
Since it is also expected that the local summation of occupied and unoccupied states results
in a constant, it would be interesting to study how the local density of states is modified
with the CDW transition.
Electronic density can be calculated from the wave function Eqn. (2.10), as the sum-
mation over all of the occupied states,
[1− 2UkVk cos(2kFx+ φ)] , (2.11)
Figure 2.3: LDOS evolution with the periodicity of CDW from mean-field theory calculation,with the horizontal axis being energy and vertical axis being real-space position. Three clearfeatures are: 1. There is a gap around EF; 2. States around EF is affected the most; 3. TheLDOS is enhanced on the filled and empty sides alternatively.
In a STS experiment, one measures density of states not only in real space but also
with energy resolution, so it is more appropriate to rewrite the density of states as follows,
|E|2 − |∆|2, (2.12)
which is very similar to the quasi-particle density of states of a superconductor (BCS theory).
This equation is only valid for |E| > |∆|, and for the energy window |E| < |∆|, there is no
density of states ρ = 0. This corresponds to the gap opening shown in Fig. 2.2.
-0.4 -0.2 0 0.2 0.4Energy
Figure 2.4: Representative LDOS curves in an electron-driven CDW. Here we have assumedthe phase φ of CDW is zero, φ = 0.
An important feature of Eqn. (2.12) is that the coefficient of the cosine term changes
its sign in between occupied (E < 0) and unoccupied states (E > 0). This results in either
enhancement or suppression of density of states on the occupied/unoccupied states, which
varies with the spatial location (relative to the CDW). Figs. 2.3 and 2.4 shows the spatial
evolution of the LDOS with the periodicity of CDW. As we mentioned in Ch. 1, the STM
imaging is not only sensitive to the positions of the ionic cores but also the electronic density
of states around the Fermi level (see Eqn. (1.6) for details). From this we can easily see
that in the presence of this spatially switching enhancement/suppression in LDOS the STM
topography will show a contrast inversion between the images of occupied and unoccupied
states (set by the polarity of tunneling bias voltage). This contrast inversion phenomenon
has been well demonstrated in various CDW systems, including NbSe3 , Sn(Pb) covered
Ge(111) surface [23, 24], CaC6 , etc.
2.2 Charge-density waves in quasi-2D materials
Quasi-2D materials that exhibit CDW states include the layered transition metal
dichalcogenide (TMD) , RTe3 , Sn (Pb) covered Ge(111) surfaces, etc. The TMD is a
wide class of materials that mainly includes two structure phases (the 2H and the 1T phases)
of many transition metal dichalcogenides. For example, 2H-NbSe2, 2H-TaSe2, 1T-TaS2 and
1T-TiSe2 are among the most studied TMDs. 2H-NbSe2 shows both superconductivity at
7 K and CDW at 35 K. 2H-TaSe2 has two CDW phases with transition temperatures at
122 K and 90 K, together with a superconducting transition at 0.1 K. 1T-TaS2 exhibits a
rich temperature-pressure phase diagram including numerous CDW phases and supercon-
ducting phase . In addition, the checkerboard phenomena in superconducting cuprates
is also argued as a strong candidate for CDW [28, 21], while cuprates are widely accepted
as two-dimensional systems.
2.2.1 Introduction to 2H-MX2
Transition metal dichalcogenides are among the earliest materials studied by scanning
tunneling microscopes [29, 30, 31, 32, 33, 34], likely due to that they are easily cleaved and
their surfaces are relatively inert even under ambient condition. In this thesis, I will mainly
focus on the trigonal prismatic structure phase (2H) of TMDs, including 2H-TaSe2, NbSe2
and TaS2. The structure of the 2H phase is fairly simple; it consists of chalcogen layers
and transition metal layers with the smallest building block being two chalcogen layers
sandwiching one transition metal layer. As shown in Fig. 2.5, the bonding between the two
adjacent chalcogen layers is of van der Waals type and thus can be mechanically cleaved.
The topmost atomic layer post cleavage can be imaged with STM, as shown in Fig. 2.5. Each
individual object is a chalcogen atom and the 3 × 3 superstructure is due to the formation
of CDW. Similar atomic resolving images of TaSe2 and TaS2 are shown in Fig. 2.6.
Figure 2.5: Topography and crystal structure of the 2H-NbSe2. (a) Topographic image ofNbSe2 surface at 5 K and 50 mV and 80 pA. (b) Crystal structure of 2H-MX2 with the dashedline indicating the cleave plane. Black/red atoms are Nb/Se. (c) A line profile indicating adiscontinuity of CDW order and visualizing the incommensurability of CDW in NbSe2.
The CDW transition in 2H-TMD have been studied in numerous experiments, including
transport and specific capacity measurements, scattering experiments (neutron, X-ray, elec-
tron diffractions, etc.), real-space imaging (STM), etc. The difference in momentum-space
electronic structure can also be measured using angle-resolved photoemission spectroscopy
Specific heat measurement of the CDW transitions in TaSe2 done by Craven et al. is
shown in Fig. 2.7 . As we can see that there is a well defined 2nd order phase transi-
tion at temperature 122 K and there is another transition at 90 K that is hysteretic and
hence 1st order. The transition at 122 K is a transition from normal state to an ICDW
(incommensurate CDW), while the transition at 90 K was thought to be a lock-in transition
from incommensurate to commensurate state (see Fig. 2.7). However, recent study with
high-resolution X-ray diffraction and better temperature control reveals a more complicated
phase diagram between 90 and 122 K .
Figure 2.6: Topography of TaS2 and TaSe2.
The CDW phases in NbSe2 and TaS2 on the other hand are both incommensurate with
respect to the lattice periodicity down to the lowest temperatures studied thus far. The
CDW wave vector in NbSe2 is measured to be qCDW = 0.328a∗ by neutron scattering, where
a∗ is the reciprocal lattice vector . In TaS2 it is observed that qCDW = 0.338a∗ by electron
diffraction experiments .
Figure 2.7: Specific heat and neutron scattering measurements of the two CDW transitionsin TaSe2. (a) Specific heat measurement shows a second order transition at 122K anda hysteretic first order transition at 90K. (from ref. .) (b) Elastic neutron scatteringmeasurement shows the appearance of two super-lattice peaks around 4/3a∗, which at lowertemperature merge into one peak sit exactly at 4/3a∗. (from ref. .)
2.2.2 Recent progresses and remaining issues
Electronic originating CDW is a natural result when one considers the different CDW
wave vectors qCDW in different materials that vary with temperature, since the most obvious
difference between them is first of all the difference in Fermi surface geometry. The incom-
mensurate behaviors in CDW further support the role electrons in the CDW transitions, due
to the general expectation that 2kF will not be a rational fraction of the lattice reciprocal
vectors. When the Fermi surface of TaSe2 is mapped out by ARPES experiment  and the
auto-correlation map is generated, a peak corresponding to qCDW was indeed found there, as
shown in Fig. 2.8.
(a) (b) (c)
Figure 2.8: Fermi surface map obtained by fitting ARPES data and possible nesting mech-anism. (a) Fermi surface obtained by fitting the ARPES data with a tight-binding model.(b) Auto-correlation map of (a). (c) Line profile along the ΓM direction. Data from: 
The purely electron-driven Peierls mechanism is a beautiful theory since it only involves
consideration about the geometry of the Fermi surface. However, the applicability of this
theory has been questioned for long time. Chan and Heine , after considering the Coulomb
and exchange interactions, concluded that a CDW is not possible when there is not periodic
lattice distortion (PLD). If there were no PLD, a CDW is never possible also because that
spin-density wave (SDW) instability will set in first. The criterion for a CDW/PLD to occur
+ (2Uq − Vq) , (2.13)
where ωq is the undressed phonon frequency, χq is the Lindhard response function, ηq is the
electron-phonon coupling strength, Uq and Vq are the Coulomb and exchange interaction.
Furthermore they found that CDW/PLD can win over SDW only when4η2q~ωq
− 2Uq > 0 and
More recently, Johannes et al., after studying the exact same systems including TaSe2
and NbSe2 using first principle calculations [42, 43], found that no CDW can be formed by
the electron systems if the ions were held in place. Their study further extends to other
materials like ErTe3 and artificial Na atomic chains with the same conclusion that lattice
distortion is a prerequisite for CDW formation.
Using inelastic X-ray scattering that directly probes the phonon dispersions, Weber
et al. discovered that in NbSe2 the phonon mode corresponding to qCDW exhibits uncon-
ventional behavior with the CDW transition . Unlike the expected cusp-shape phonon
softening near qCDW , the phonon energy was reduced to zero over an extended range
of q vector. This is more consistent with a wavevector-dependent electron-phonon coupling
which is capable of driving a structure phase transition.
Figure 2.9: Phonon anomaly in 2H-NbSe2. The extended region where the phonon energy isreduced to zero cannot agree with conventional fermi surface nesting related Khon anomaly.Data from 
Another difficulty with the applicability of Peierls mechanism in 2H-NbSe2, TaSe2 and
TaS2 lies in the results of transport measurements (see Fig. 2.10). All three of the materi-
als show kinks in ρ(T ) at the CDW transition temperatures that indicate better electrical
conductivity in the CDW phases. This directly conflicts with the prediction of Peierls mech-
anism that an energy gap should open up at the Fermi level and the system becomes an
insulator. This could be explained if the CDW state is carrying electrical current as the
cooper pairs in a superconductor. However, the pairing in a CDW is between electrons and
holes  which is charge neutral. Furthermore, the lattice distortion associated with the
CDW also prohibits it from sliding freely, making it impossible to contribute to the increase
of conductivity. The enhancement of electrical conductivity in these compounds at TCDW
has remained mysterious thus far, to the knowledge of the author.
5 10 20 50 100 200
RRR = 10
RRR = 30
RRR = 50
RRR = 60
RRR = 100
Figure 2.10: Conductivity enhancement with CDW transitions in 2H-MX2. Data from and .
It has also been reported that resistivity anisotropy increase with a larger slope with
respect to temperature in the CDW phases [46, 47]. It appears like the CDW transitions
alter the in-plane electronic scattering mainly. In TaSe2, the electronic scattering rate from
the Drude term follows the same trend as the resistivity . From thermal transport
measurement in NbSe2, a large Nernst singal has been observed in the CDW state ,
which also points to a change in the electronic scattering along with the transition.
Shown in Table 2.1 is a summary of the transition temperatures of both CDW and
superconductivity in four 2H-TMDs. The CDW transition temperatures are much higher
with the Ta compounds, and superconductivity transition temperatures are much higher
Table 2.1: CDW and superconductivity transition temperatures of 2H-MX2
TaSe2 TaS2 NbSe2 NbS2
TCDW (K) 122 78 35 no CDWTC (K) 0.1 0.8 7.2 6.1
with the Nb ones. Among the differences between niobium and tantalum are that Ta has
5d electrons and Nb is the 4d counterpart and that Nb has slightly higher electronegativity.
It is also known that in NbSe2 the metal ion is not fully tetravalent and the Fermi surface
comprise a small pocket of Se p band , while it is not the case for TaSe2 . Do
5d electrons favors CDW while 4d electrons favor superconductivity? Are electron-phonon
coupling dominating these transitions? Our STM results (Figs. 2.5 and 2.6) show that the
CDW in Ta compounds is more rigid compared to NbSe2, in which long range CDW order is
often interrupted. This could not be due to different impurity levels in the sample growing
processes, since the STM images show no direct relation between the atomic defects and the
defects in CDW superstructures. However, within the system of NbSe2, Iwaya et al. indeed
reported that Ta dopants disturb the CDW order .
2.2.3 CDW gap opening
One of the most prominent signature of a Peierls type CDW is the opening of an energy
gap around the Fermi level. In 2H-TMDs the search for such kind of a gap has been very
frustrating for physicists. Three of the most commonly used methods are single-particle
tunneling experiments, optical conductivity measurement and angle-resolved photoemission
spectroscopy. These experiments give results that are not in agreement.
An early study by Hess et al. in NbSe2 revealed the kinks at 35 meV in tunneling
dI/dV spectrum, which were then attributed to the CDW formation Hess . Firstly, the
the finite density of states around zero bias voltage means the gap opening is not around the
entire Fermi surface. Secondly, the measured gap value of 35 meV seemed to be too large for
mean-field theory to be applied; 2∆/kBTCDW = 23.3 which is one order of magnitude larger
than the predicted value from mean-field calculation, 2∆/kBTCDW ≈ 3.52 . Recently, it
has been reported that this 35 meV gap persists at temperature above TCDW , indicating
that it is probably not the correct CDW energy gap.
Figure 2.11: Local density of states measurement on NbSe2, showing the two kinks at ±35mV measured at 4 K (red arrows). The lower part shows the superconducting gap measuredat 50 mK. Data from .
ARPES experiments, capable of resolving band structure in the k−space, have reported
momentum-dependent gap structures across the Fermi surface for many 2H-TMDs [40, 50,
52]. For TaSe2, there is a k−dependent pseudogap which reduces with increasing temperature
but persist up to room temperature with the gap value varying from 10 to 40 meV. In NbSe2
there is also a similar k−dependent gap opening with gap value ranging from 2 − 6 meV.
Despite their difference in gap values, there is one interesting common feature between TaSe2
and NbSe2; the gap values are larger on the Fermi surface segments closer to K-point of the
Brillouin zone and are smaller or zero on points closer to M-point or Γ-point. Studying the
complicated gap formation in k−space might lead towards understanding of not only the
CDW problems themselves but also other correlated behaviors of electrons.
Another commonly used experiment that can determine the gap size is by measuring
the optical conductivity or dynamics. From both the dynamics study by Demsar et al. 
and optical conductivity study by Vescoli et al. , gaps of 2∆ = 70 meV have be measured
in TaSe2, although their gap-temperature dependence are not in agreement.
2.2.4 Doping and superconductivity
Figure 2.12: Phase diagrams of Cu intercalation into TiSe2 (a) and TaS2 (b) (Cu2TiSe2 andCuxTaS2), from [54, 55].
Intercalating dopants into the space between the chalcogen layers bonded by van der
Waals force usually introduces interesting changes to the physical properties of the layered
structure materials like TMD . For example, intercalation of copper into 1T-TiSe2 and
2H-TaS2 have both resulted in superconductivity with Tc above 4 K (CuxTiSe2  and
CuxTaS2 ). Their doping phase diagrams (Fig. 2.12) are very similar to that of high-Tc
superconducting cuprates  and pnictides with CDWs replaced by pseudogap, antiferro-
magnetic or spin-density wave phases.
Not only metals can be intercalated into the van den Waals gaps of the layer-structured
materials, (organic) molecules can do very similar things . An interesting fact is that
methylamine (CH3NH2) intercalated TaS2 has the highest superconducting transition tem-
perature (Tc = 5.6 K) among the intercalation compounds of TaS2. The dimensionality
change due to intercalation or the suppression CDW order caused by the disorder is proba-
bly responsible for the rising of superconductivity in these materials.
More interestingly nickel dopants in NixTaS2, which is also superconductor (Tc = 4 K),
have been reported as replacing Ta instead of intercalation between the S-Ta-S sandwiches
. Atomic resolving STM imaging could serve as a powerful tool to distinguish between
these two cases. Furthermore, studying the different intercalating/substituting dopants with
respect to the reminiscent CDW order will be helpful for studying the microscopic origin of
the CDW in the TMDs.
Charge-density wave is a long-standing topic in condensed matter physics and yet is
still a very intriguing and puzzling one, which is closely related to other topics like high-Tc
superconductivity, colossal magneto-resistivity, etc. In the 2H-TMDs, the driving force of
the CDW transition is still under debate, while many experimental facts (e.g. transport and
phonon) have clearly shown their unconventional behaviors compared to 1D CDW systems.
Using an atomically resolving STM, together with its high energy resolution of measuring
local density of states of both the occupied and unoccupied levels, seems to be a promising
tool for understanding the microscopic physics of charge-density waves in the 2H-TMDs.
Together with the recently reported data from ARPES and high-resolution scattering exper-
iments, we will try to push the understanding of TMD-CDW systems to a better level.
Strong periodic lattice distortion in 2D charge-density wave systems
In condensed matter physics only a handful of models have both elegance in their
construction and are thought to describe the behavior of numerous materials. The Peierls
transition , for electrons crystallizing into charge-density waves (CDW), is one such
model that has been successfully applied to many 1D systems . However, in the quasi-2D
electron systems of the layered transition metal dichalcogenides (TMD) there is still a con-
troversy about the nature of the transitions to CDW phases, i.e. whether they are described
by a Peierls-type mechanism or by a lattice driven model. By performing scanning tunneling
microscopy (STM) experiments on the canonical TMD-CDW systems, we have successfully
imaged the electronic modulation and the lattice distortion separately for the first time.
Across three materials (2H-TaS2, TaSe2, and NbSe2), we found dominant lattice contribu-
tions instead of the electronic modulation expected from Peierls transitions, in contrast to
the CDW states that show the hallmark of contrast inversion, in 2D [23, 24, 25] and 1D
 systems. Our results imply that the periodic lattice distortion (PLD) plays a vital role
in the formation of CDW phases in the TMDs, which is in agreement with the theoretical
studies [41, 42, 43], especially recent work by Johannes et al. [42, 43]. Our results illustrate
the importance of taking into account the more complicated lattice degree of freedom, and
they will prove useful in the studies of other correlated electron systems.
The CDW instability in low dimensional systems was initially explained by the Peierls
transition [59, 12] in which a divergence in electronic response function at a particular wave
vector (2kF for 1D) results in a periodic charge redistribution in real space. That is, a low
dimensional electronic system can lower its energy by opening an energy gap at the Fermi
level, piling up electrons periodically and reducing its lattice transitional symmetry. As
a result of the periodic electron modulation (eMod) and the electron-phonon interaction,
the lattice itself undergoes a similar modulation, which causes an increase in the lattice
elastic energy . As a consequence, the lattice distortion will be minimized and acts as
a secondary effect . The eMod is embedded in the change of the local density of states
(LDOS), which we have calculated for real-space from the Peierls model (Supplementary part
I). Another way of visualizing the problem is by using the sum rule in quantum mechanics,
where the summation of the numbers of filled and empty states on every lattice site is a
constant. So that wherever there are excess electron states, there will be less hole states on
the same site. The LDOS calculation we have performed also shows the conservation of total
The tunneling current in a STM junction is proportional to the sample’s integrated den-
sity of states and a matrix element with exponential dependence on the tip-sample distance,
I ∼ e−2κs∫ eV
0LDOS(ǫ)dǫ . In the constant current imaging mode, the tunneling current is
maintained at a fixed value with the tip-sample distance being adjusted and recorded. For
a CDW system that only contains eMod and no lattice distortions (like the one in Fig. 2.3),
the topographic image of the filled states will be complementary with the empty states due
to the nature of LDOS variation and uniformity of atomic positions. Therefore, the constant
current height images of filled and empty states, in such a CDW system, will accordingly
be complementary. This phenomenon has been well demonstrated by STM experiments on
many CDW systems (see next Section for details). In each of these cases the modulations,
with the CDW periodicity, are of opposite phases for electron- and hole-like states in the
topography. This is predicted for a Peierls transition.
3.2 Previous STM study of topography in CDW systems
Filled states Empty states
Figure 3.1: Previous STM images of Ge(111) surface covered by 1/3 monolayer of Sn, showingthe contrast inversion of topography between filled and empty states. Images were taken with∓1V for filled/empty states at room temperature (upper) and low temeprature (lower). Theimage on the right is an averaged image between the two images taken at low temperature,which fully recovers the atomic order with no super-lattice structure. Data from .
As we mentioned in Ch. 2 and in the previous section, a hallmark of the CDW phase
is the contrast inversion between images of filled and empty states; the electron-like states
are redistributed in a periodic manner, namely charge-density wave. At the same time,
the hole-like states will also be redistributed but with an opposite phase; the summation
of electron-like and hole-like states on a particular lattice site has to be conserved. This
hallmark contrast inversion phenomena have been reported on many different CDW systems,
including the quasi-1D NbSe3 (Fig. 3.2 ), the 2D systems of Sn/Pb covered Ge(111)
surfaces (Fig. 3.1 [23, 24]), and the quasi-2D CaC6 with 1D modulation .
In the two-dimensional systems of Sn/Pb covered Ge(111) surface, the triangular lattice
of Sn/Pb atoms show a uniform atomic lattice at room temperature. Upon cooling to
low temperature, both Sn and Pb systems exhibit a reconstruction with√3 times larger
lattice periodicity (Fig. 3.1). More importantly, STM imaging showed that the filled and
empty states were perfectly complementary, indicating the reconstruction is with valence
electron redistribution instead of lattice distortion, which is predicted as a charge-density
wave. However, detailed study about the electronic structure in the framework of Fermi
surface nesting were not able to predict this charge instability , implying the limitation
of nesting related CDW origins.
Figure 3.2: Previous STM images of NbSe3 cleaved along (b, c)-plane, with b being the chaindirection. The size of these scans were 7 × 7 nm2. (a) and lower side of (b): topographicimage with +200mV. Upper side of (b) and (c): topographic image with −200mV. The bluelines are guides for the contrast inversion along the chain direction. Data from .
In NbSe3, a one-dimensional chain compound that exhibits two CDW transitions at
low temperatures, very similar contrast inversion has been observed by Brun et al., as shown
in Fig. 3.2. In this material, there are three types of one-dimensional chains (type I, II and
III in Fig. 3.2), lying along the b-axis. The features along the chain direction are the CDW
minima and maxima. With the blue lines indicating the same locations in different images,
we can clearly see the inversion of apparent height between the images of filled and empty
states (∓200 mV).
3.3 Strong lattice distortion in 2H-MX2
The TMDs (e.g. 2H-NbSe2, TaSe2, 1T-TaS2, and TiSe2) have drawn a lot of atten-
tion due to the coexistence and competition between the CDW and the superconductivity
phases which are induced by the complicated interactions between the internal degrees of
freedom, including charge, lattice and orbital [54, 55, 27, 60]. However, whether or not an
electron-driven mechanism can be the cause of the formation of CDWs in the TMDs with
the trigonal prismatic structure (2H) is still under debate. The existence of incommen-
surate CDW phases does lend support for the role of electronic interactions as the cause,
since 2kF is generally not expected to be a rational fraction of the lattice reciprocal vectors.
Furthermore, the electronic origin is also supported by photoemission experiments [40, 50].
By measuring the Fermi surface with ARPES and calculating the electronic susceptibility
through the autocorrelation, peaks were found at wave vectors corresponding to those of the
CDW [40, 50]. However, inelastic X-ray scattering experiment  reveals that the lattice
dynamics exhibit unconventional behavior and hence may be dominating the transition. In
a recent real space study, Soumyanarayanan et al.  have shown that there is a close rela-
tionship between CDW formation and the local strain related to the surface layer buckling
in NbSe2. Furthermore, existing studies have proposed a variety of different mechanisms,
including the Fermi surface nesting , saddle band driven susceptibility divergence ,
f-wave gapping and marginal Fermi liquid , etc. Rossnagel et al. has, in addition, ar-
gued that the spin-orbit interaction is also important for 5d-electron materials like TaSe2
and that the band structure calculation is able to reproduce k-dependent gap structure .
Moreover, recent LDA calculations have shown the difficulties with Fermi surface nesting
and have suggested that PLD, instead of eMod, is the essential ingredient [42, 43]. Because
of this debate, it is necessary to study the nature of the 2D CDWs in the TMDs with the
simultaneous measurement of any intrinsic lattice distortion while spatially resolving the
electronic component across this family of compounds.
We have examined three 2H-TMDs, TaS2, TaSe2, and NbSe2. Figure 3.3a is a repre-
sentative constant current topographic image of a 2H-TaS2 surface showing both the atomic
corrugation and the 3×3 CDW superlattice. TaS2 is being studied here for the first time by
a STM. Fig. 3.3b shows crystal structure with the neutral cleave plane (dashed line) between
the two layers of chalcogen atoms. The atomic lattice shown in Fig. 3.3a is the resulting
Figure 3.3: (a) Atomically resolved topographic image of 2H-TaS2 with CDW modulation(3×3 superstructure). This image is obtained at 60 K and with setup condition being−100 mV and 200 pA. Inset: zoom in to show the atomic structure of the 3×3 unit cellwith red circles indicating the sulfur atoms. (b) Crystal structure of trigonal prismatic (2H)TMD. The red/black atoms are chalcogen/metal atoms, and the dashed line is where itcleaves. (c) Fourier transform of (a). Blue (red) circles indicate the primary peaks of CDW(atomic) modulation, and b1 and b2 are the atomic lattice reciprocal vectors.
triangular chalcogen lattice, while the evident 3×3 superlattice is due to the formation of
the CDW. The Fourier transform (Fig. 3.3c) of Fig. 3.3a shows that the atomic and the
CDW signals are the main features of this surface. After excluding the atomic corrugation
by Fourier filtering, we find that the height of the top layer of atoms changes on the order
of picometer in the z direction due to the formation of CDW, for all three of the 2H-TMDs.
This change is consistent with the distortion measured by both x-ray diffraction  and
neutron scattering experiments . This agreement strongly indicates that our surface
sensitive measurements of the CDW show similar behavior as the bulk.
In order to probe the differences between the electron and hole (filled and empty)
states of the CDW phases in these materials topographic images were taken at opposite
sample biases. In Figs. 3.4 and 3.5, our topographic images obtained on 2H-TaS2, NbSe2
and TaSe2 are shown. Figs. 3.4a and 3.4b are images of the filled and empty states (as
indicated by negative and positive sample biases) in TaS2 while Figs. 3.5a-b and 3.5e-f are
images of the empty and filled states in NbSe2 and TaSe2. Prior to analysis, these images
are processed with a drift-correction algorithm  so that images taken at different times
can be aligned on a subatomic length scale. The surface defects are used to ensure accuracy
of the drift correction algorithm. This process, combined with the high thermal stability of
our experiment, allows for an extremely precise measurement of position (with less than 50
pm of drift per day) and enables us to uncover the true structure of the CDW state in these
materials for the first time.
Comparing our results with those from known CDW systems [23, 24, 22], which in-
clude STM results on NbSe2 , we find qualitative discrepancies. In our measurements,
the filled/empty states topographic images of the TMD samples do not show the expected
out-of-phase or spatial “inversion” that the Peierls model predicts. This contrasts with pre-
vious observations of 2D systems such as Pb (or Sn) coated Ge(111) [23, 24]. Instead, the
topographic images taken at +50 and -50 mV sample bias voltages on TaS2 are very similar
to each other when one compares them with the naked eye. In order to rigorously check this
302520151050Lateral position (Å)
Figure 3.4: Topographic images showing symmetrization and antisymmetrization on 2H-TaS2 at 52 K. (a) and (b): Topographic images with −/+50 mV and 100 pA. These twoimages were individually corrected for drift and aligned with sub-atomic precision. (c) and(d): The symmetrized (S = (a+ b)/2) and anti-symmetrized (AS = (a− b)/2) images of (a)and (b). The contrast in (d) is much smaller compared to (c). (e): The line profiles in (a-d)indicated by colors.
similarity, we have calculated the normalized cross correlation coefficients (NCC) between
two images (Aij and Bij),
NCC =〈(Aij − µA) (Bij − µB)〉
where µA and µB are the average values of the two images and σA and σB are the standard
deviations. NCC is expected to be +1 for two identical images, and −1 for two images
with perfect contrast inversion. For an eMod-dominating CDW, where spatial inversion
between filled and empty states is expected, such as Pb/Ge(111), one would expect the
NCC between the filled and empty states images to be close to −1. What we find when
we carry out this analysis on TaS2, NbSe2 and TaSe2 is that the NCCs are +0.62, +0.79
and +0.95 respectively, showing that the majority of the topographic images are in-phase
between the two biases. Considering that only the CDW corrugation will be out-of-phase
while the atomic corrugation is actually in-phase, we can remove the atomic signals by
Fourier filtering them and keep only the CDW signal. After removing the atomic signals,
the measured NCC are still +0.37, +0.67 and +0.97 for TaS2, NbSe2 and TaSe2 respectively,
in sharp contrast to the −1 expected for a traditional CDW. It is important to note that this
result differs from previous STM results on NbSe2  where spatially out-of-phase electron
and hole components were seen. This discrepancy is due to our superior ability to control
and correct for drift at the subatomic level which allows us, for the first time, to uncover
the true nature of these materials. Interestingly our measured positive valued NCCs do not
agree with the conventional pure electronic CDW model  and instead show that there is
another non-electronic, lattice effect that is important to the formation of the 2D CDW in
PLD is a natural explanation for the positive NCCs we measure since STM measure-
ment is a combination of the atomic structure (via the tip-sample distance) and the integrated
density of states. If the ionic cores, around which the valence electron clouds are centered,
are displaced with the CDW transition, i.e. lattice distortion occurs, then the filled-state and
Figure 3.5: Topographic images of NbSe2 and TaSe2 at 5 K. (a/b): Topographic images ofNbSe2 with −/+100 mV and 100 pA. (e/f): topographic images of TaSe2 with −/+50 mVand 40/30 pA. (c/g) and (d/h): Symmetrized and antisymmetrized images of (a/e) and(b/f). The contrast of (c/g) is much larger than (d/h), same as TaS2.
empty-state topographic images will be in-phase with each other. This is because they only
enter into the tunneling current through the electron-hole symmetric matrix element. In
other words, if there is only a periodic lattice distortion then the filled-state and empty-state
topographic images will be the same, except with a possible difference in the amplitudes of
the height profiles, which will not affect the NCC. This is exactly what we see in our STM
images of the 2H-TMDs.
By calculating the symmetrized (Figs. 3.4c, 3.5c and 3.5g, S = (a + b)/2 where a
and b are the images of filled and empty states) and anti-symmetrized (Figs. 3.4d, 3.5d
and 3.5h, AS = (a − b)/2) images, we can directly access the PLD and eMod parts of the
data respectively. Results of these calculations, shown in Figs. 3.4 and 3.5 using the same
height scaling, clearly show that the symmetrized channel has a larger z-range than that of
the anti-symmetrized one, agreeing with our measured NCCs above. The two channels (S
and AS) reveal the decomposed, spatially resolved, PLD and eMod components of the 3×3
superlattice for the first time. We find similar signals for the two other members of the 2H
family that we have measured, NbSe2 and TaSe2. In the framework of Peierls instability, the
lattice distortion acts as a secondary effect which has to be minimized because it increases
the elastic energy of the ground state. Contrasting with the results of the previous STM
study , we have demonstrated that the PLD is playing an important, if not the primary,
role in the CDW formation in 2H-TMDs. This is calling out a strong entanglement of the
PLD and the eMod, which is not to be expected in a purely electronic Peierls picture.
Our results agree with the calculations which show that without the lattice involvement
a CDW in these systems cannot exist. It has long been argued that without lattice distortions
electron correlations are too strong for a purely electronic CDW to form  and that there
must be corresponding lattice distortions. Our observations clearly show that these lattice
distortions are present and dominate the observed structure in the 2H-TMDs, which is in
contrast to previous reports to the contrary . In addition, recent theoretical calculations
in this family of materials have shown that the observed CDWwave vectors do not correspond
Figure 3.6: Topographic images on 2H-NbSe2 at T = 6 K. Scan size is about 20 × 20 nm2.(a) and (b): Topographic images with -50 mV and +50 mV. (c) and (d): Symmetrized andanti-symmetrized image of (a) and (b).
to the peaks in the electronic susceptibility . This calls for a more complicated model
that includes nontrivial phonon involvement. Such complicated origins of the charge ordering
transition in such a simple family of materials demonstrates the necessity of taking the lattice
contribution into account in describing the phase diagrams of everything from the simple
systems like TMDs, to the more complex correlated electron materials like cuprates and
The symmetrized topographic images do not contain the eMod signal because the
eMod will cause asymmetric changes in LDOS (Fig. 2.4 in Ch. 2). Instead the symmetrized
topographic images contain the PLD signal since it symmetrically affects the filled and
empty states. It is possible, however, that the anti-symmetrized images do contain more
information than just that of the eMod. In this sense, the relative intensity of PLD versus
eMod we present is only a lower bound on the lattice contribution to the CDW. As we
mentioned earlier, the topography is only sensitive to the energy window which is set by
tunneling bias voltage, so high energy studies might reveal a more complete picture of CDW
in 2H-MX2. However, even with our low bias voltage images presented here, our study
presents more than enough evidence to show the violation of the Peierls picture in the 2D
CDWs in these materials. Furthermore, we have indeed checked these results by measuring
over a range of bias voltages form 25 to 200 mV and have seen no inconsistencies.
3.4 Topographic images on CuxTaS2
We have further extended our study to Cu intercalated TaS2 sample, CuxTaS2 (x =
0.04). In this sample, the copper atoms sit inside the van der Waals gap between the two
S layers, and after cleavage they shows up as ad-atoms on the surface (Fig. 3.7a). Our first
finding was that the copper dopants largely disturbs the 3 × 3 super structure (weakening
the CDW order) which is consistent with the reduction of CDW transition temperature by
copper intercalation .
These copper atoms are mobile under the strong electric field inside a STM tunneling
Figure 3.7: Topographic images with various bias voltages on CuxTaS2 (nominal dopingx = 0.04) at T = 6 K. (a) A large area (120 × 120 nm2) scan of the CuxTaS2 surface. (b-e)Images of the same area with various bias voltages, after the copper atoms were moved awayfrom this area.
junction and therefore can be manipulated by the tip. To help understanding the role of
copper atoms in the reduction of CDW order, we then removed ‘all’ of the copper from a
small area. The removal of the surface copper does not recover the long range 3 × 3 order
as those in pristine TaS2, which points the local disorder to the Cu buried underneath the
first sandwich layer of S-Ta-S.
This further allows us to check for the lattice distortion in such a disordered CDW
system. Figs. 3.7b-e show the topographic images of this area with different bias voltages.
It is easy to observe that these four topographic images look very similar to each other
except the change of overall contrast. The change of overall contrast is also consistent with
the undoped samples. The similarity between these images prove two things: 1. the PLD
is playing the major role again in this disordered CDW system; 2. the copper atoms are
likely not substituting the Ta due to the atomic uniformity at all bias voltages. Moreover,
we found that the local CDW order is not changed very much before and after the surface
layer copper atoms were removed, indicating that the copper atoms are altering the CDW
by creating the local strain instead of charge doping. The absence of charge doping is also
confirmed by the weak bonding between the copper and TaS2 (easiness of moving the copper
around the surface).
In summary, we have demonstrated the importance of a high resolution, high stability,
low drift STM to the understanding of the structure and origins of CDWs in the TMDs.
We have shown that atomic length scale measurements are necessary in order to resolve
and separate the structures of both the PLD and eMod in TaS2, NbSe2 and TaSe2. This
shows that the PLD dominates the CDW transition for the entire family of 2H-TMD and
that the eMod, which has been previously been seen as the dominating mechanism, plays
a secondary role instead. These conclusions were further confirmed by data from a copper
doped TaS2 sample. Our results indicate that pure electron driven CDW is unlikely to exist
in the 2H-TMDs and that the PLD plays an important role, which is in excellent qualitative
agreement with the recent theoretical studies .
Orbital-cooperative CDW transition in 2H-MX2
The charge-density wave (CDW) transition breaks the lattice translational symmetry
and piles up electric charge periodically in real space. In the simplest model for this, Peierls
 pointed out that this transition, purely driven by electronic instability, will lower the
energy of electrons by opening up a gap at the Fermi level and driving the system from
metallic to insulating state. After being successful with many 1D charge/spin density wave
systems , this model itself and similar ones which rely on Fermi surface nesting have been
widely applied to correlated electron systems [19, 67, 21, 20]. However, a good understand-
ing of the two dimensional charge-density wave (2D-CDW) in the layered transition metal
dichalcogenides (TMD, MX2)  is still lacking leaving many unanswered questions. For
instance, enhancement of electric conductivity with the CDW transition has been reported
for many MX2 systems including 2H-TaSe2, TaS2 and NbSe2 [35, 46, 60, 45], opposite to
the prediction of Peierls mechanism. Partial gapping on Fermi surface  is only able to
explain the metallic state below TCDW, but not the enhancement of conductivity. The sliding
CDW picture also lacks direct experimental support for these 2D systems. Moreover, mea-
surement of the Nernst effect on NbSe2  also gave surprisingly large signal accompanying
the CDW transition that has not been fully explained. These unconventional properties call
for alternative explanations for the 2D-CDW in the TMDs. From theoretical perspectives,
challenge to the Peierls mechanism has been brought up by Chan and Heine , who ar-
gued that a CDW cannot be stable without lattice distortion. Recent work by Johannes et
al. [42, 43] further suggests that the low-energy approximations, like the BCS-type mean
field calculation , are not enough to describe the TMD-CDW systems, and states away
(≫3.5kBTCDW) from the Fermi level are also important for the transition. Furthermore, van
Wezel  has pointed out that orbital degree of freedom could play an important role for
Figure 4.1: Band structure of TaSe2 from first principle calculation (black and blue opencircles). The color of the circles indicate the characters of dz2 (black) and dxy/dx2−y2 (blue)orbitals. From: ref. 
Two dimensional charge-density wave (CDW) materials like 2H-TaSe2 and TaS2 belong
to the multi-orbital correlated systems, similar to manganites , Fe-based superconductors
, ruthenates , iridates , etc. According to theoretical calculations [70, 75, 76], the
conduction band is composed of three hybridized d-orbitals, with the dz2 at the center and
dxy/dx2−y2 on the edges of Brillouin zone. These calculations have been confirmed with
Fermi surface measurements by ARPES . The orbital texture of the conduction band
has been argued as nontrivial . However, to date there has been no experimental report
on the orbital structure of the energy bands, likely due to the complicated structure of the
particular d-orbitals involved here. Fortunately, the dramatic difference expected in the
spatial extension of dz2 and dxy/dx2−y2 orbitals offers an excellent opportunity for real-space
resolving probes to look for their ordering. One such probe, spectroscopic imaging scanning
tunneling microscope (SI-STM), measures electronic density not averaging the entire sample
but the component that extends into the vacuum by 5-10 A , where tunneling process
can occur but no significant perturbation to the intrinsic property is induced by the tip.
With a simple atomic limit model (see supplementary information), we have shown that
the exponential decay length of dz2 is much larger than for the dxy/dx2−y2 states leading to
a much larger overlap at the location of the STM tip. Therefore LDOS measurement will
sample dz2 more than dxy/dx2−y2 orbitals allowing a spatial mapping of the different orbital
states. Moreover, STM is able to image the periodic lattice distortion and the electronic
component of the CDW state separately (see Ch. 3), and its LDOS measurement covers
both filled and empty states.
Among the existing studies of 2H-MX2 the change in local anion coordination of metal
atoms with CDW formation are rarely taken into account, due to the small amplitude and
difficulty to be measured precisely . In previous work with STM topographic images, we
were able to measure the lattice distortion directly (see Ch. 3). Since the 5d orbitals are
spatially extending and thus the crystal field effect is strong, we argue that the small amount
of lattice distortion is important, by proving a positive correlation between the local anion
distortion and energy level shifts measured from LDOS.
4.2 Averaged LDOS on TaSe2 and TaS2
To investigate these issues we have carried out STM and STS experiments on 2H-TaSe2
and TaS2 at various temperatures. Here, we present spatially averaged LDOS spectra in both
materials and address on the kink feature that has been ascribed as the CDW gap in the past
. We then use the unique ability of SI-STM to study the atomically resolvable LDOS
on TaSe2 and show the intra-unit-cell LDOS variation and its relation with the local lattice
distortion. Comparable results on TaS2 will also be presented.
In order to verify whether there is a gap formation with CDW, we have measured the
LDOS by differential conductance (dI/dV) measurement with the standard lock-in method.
-200 -100 0 100 200
-50 0 50(mV)
-200 -100 0 100 200
-200 -100 0 100 200
(a) (b) (c)
Figure 4.2: Average LDOS spectra of TaS2 at 52 K, TaSe2 at 77 and 5 K. The short verticallines indicate the locations of the kink features (−50 and +60 mV for (a), ∓50 mV for (b)and ∓30 mV for (c)). Inset of (c): zoom-in to the low energy features at ±30 mV and ±10mV. A linear background is subtracted from the raw data.
LDOS spectra in TaS2 and TaSe2 (Fig. 4.2a-c) show very similar overall asymmetry, with the
negative bias side being almost constant and positive side increasing quickly with voltage.
Around zero bias, all of our spectra display some dip features with roughly symmetric kinks
on both sides of the dips (indicated by the black vertical lines). For TaSe2 at 5 K, the
kinks in the LDOS occur at ±32 meV which is almost identical to the energy scale of a
similar feature reported on NbSe2 [34, 51]. The similarity of these features in these two
different materials is surprising if they are related to the CDW transition, since their TCDW
differs by a factor of 3 (122 K for TaSe2 and 33 K for NbSe2). According to mean field
calculation , the size of CDW gap should be proportional to TCDW (2∆ = 3.5kBTCDW).
Furthermore, as the temperature approaches TCDW, one expects the energy gap to decrease,
in sharp contrast to our observation that their energy increases with increased temperature
(Fig. 4.2b-c). Additionally, the low temperature LDOS in TaSe2 includes two more kinks
at ±10 meV within the dip, which have never been reported. All of the evidences stated
above do not support the 32 mV feature being the CDW gap. Soumyanarayanan et al. 
have also shown that these kinks do not vanish above TCDW. Instead of being related to
the CDW, an interesting possibility is that the kinks in LDOS can be explained by phonon
assisted inelastic tunneling, which is indeed able to give rise to weak step-like increase in
LDOS , and phonon density of states of NbSe2 and TaSe2 do share strikingly similar
energy scales around 10 and 25 meV [44, 76].
-800 -400 0 400 800VBias(mV)
Se p-band Ta d-band
Figure 4.3: A high energy LDOS obtained by averaging 3600 spectra taken over an area of 4× 4 nm2 and junction setup at −200 mV and 40 pA. The fast rising at −400 mV originatesfrom the Se p-bands, and the hump around +380 mV indicates a van Hove singularity inthe Ta d-band with dz2 orbital characteristics.
A major feature in the LDOS spectra is the large asymmetry between filled and empty
states. Asymmetry is common in tunneling experiments but its origin differs in each case so
material details are necessary . To study the asymmetry in TaSe2 we firstly measured
LDOS in a larger energy range. In the high energy LDOS (Fig. 4.3), two large features
can be observed and related to the energy bands . The first feature is the fast rising
below −400 mV originated from the Se p-bands, since Se atoms are closer to the tip and
thus enhanced in the tunneling process. The second one is the big hump around +380
mV, the edge of which extends towards the Fermi level and results in the ‘asymmetry’ seen
around zero bias. We identify this hump with the van Hove singularity around the Γ-point
with dz2 characteristic. As we previously discussed the dz2 orbital will be enhanced in STS
measurements in addition to the expected enhanced DOS from a van Hove singularity. Due
to the fact that conduction band gradually shifts its weight between dz2 and dxy/dx2−y2
orbitals and also the kz dispersion, the broad nature of the feature seen around +380 mV in
STS rather than a narrow one is expected.
4.3 Spatially resolved LDOS study on TaSe2 and TaS2
To further study the LDOS asymmetry, we have also measured the LDOS on a 96 × 76
pixel grid over an area of 5 × 4 nm2 with the tunneling junction set at −200 mV and 300 pA,
and we found that the asymmetry in LDOS varies in a subtle fashion with the periodicity
of the 3 × 3 CDW superlattice. To quantify this asymmetry, we have calculated the ratio
map (Fig. 4.4a) of hole versus electron density of states,
R(r, V ) =
LDOS(r, ǫ)dǫ , (4.1)
where r denotes the two spatial coordinates. The ratio map indeed reflects the same periodic-
ity with the topographic image (Fig. 4.4b), and there is no further inhomogeneity associated
with any larger length scales. It became reasonable to focus on one CDW unit cell (drawn
as the red diamonds in Figs. 4.4a, 4.4b and inset of 4.4c) and plot out the LDOS of differ-
ent high symmetry points (defined in the inset of Fig. 4.4c) within. The major difference
between the spectra is the variation of the overall slope (Fig. 4.4c). The normalized spectra
(Fig. 4.4d) show no evident energy feature within the energy window of ±200 mV, implying
that higher energy states are responsible for the CDW formation . The lack of any fea-
ture around ±32 mV in the normalized spectra further supports that the kinks (Fig. 4.2a-c)
are not related to CDW, since the BCS-type mean field calculation predicts the dominant
change in LDOS to be at ±∆ (see Fig. 2.4 in Ch.2).
More interestingly, we found that the ratio map is anti-correlated with the height map
(topography): the ratio is high when the tip height is low and vice versa. The normalized
cross-correlation number is −0.65. Considering the multi-orbital involvement [70, 75, 76], we
have established a strong relation between the change of LDOS asymmetry R(r) and the local
anion distortion. The lattice distortion occurs with Σ1 symmetry  in which the metal ions
only move within the basal plane, and chalcogen atoms move in a mirror symmetric manner
about the metal layer. Topographic image at −100 mV with the atomic corrugation filtered
out (Fig. 4.5b) can be adopted to represent the distortion of the chalcogen atoms along
-200 -100 0 100 200VBias(mV)
Figure 4.4: Ration map and sub-unit-cell LDOS variation in TaSe2 at T = 5 K. The scansize is 4 × 5 nm2. (a) R-map as defined in Eqn. (4.1), with V = 200 mV. (b) Concurrenttopographic image. Cross correlation number with (A) and (B) is −0.65, indicating ananti-correlation between them. (c) Averaged LDOS spectra over the equivalent sites of allthe CDW unit cells. Inset: definition of point of interest (POIs) using the contours withdifferent colors. POI 1−8 correspond to the colors from red to violet in a rainbow colorscheme. LDOS spectra in (c) follow the same false color scale. (d) Same LDOS spectra in(c) normalized by the average LDOS of the entire region.
z-axis. Shifts in the angle between the M-X bond and z-axis (α in Fig. 4.5a) should predict
shifts in the energy difference between dz2 and dxy/dx2−y2 . When the angle α increases (left
prism in Fig. 4.5a), the energy of dz2 (dxy/dx2−y2) will decrease (increase) and vice versa,
similar to the Jahn-Teller effect. Within this picture the correlation between the height of
chalcogen atoms and the corresponding LDOS asymmetry becomes natural. As shown in
Figs. 4.4a and 4.4b, the ratio is enhanced in the left half of the CDW unit cell indicated
by the diamond, which corresponds to a lowered dz2 level (and hence lower shoulder near
the Fermi level) with the increased angle α (Chalcogen atoms move towards the Ta layer).
The opposite situation is seen on the right half of that unit cell. The horizontal shift of the
edges at +150 mV gives an approximate change in the local energy of the dz2 band, which
is about 12 meV from lowest to highest. Interestingly, this value is very close to kBTCDW of
TaSe2. This altering of the energy levels of the different orbitals in such a spatially periodic
manner will accordingly result in a population imbalance between them, namely a partial
Figure 4.5: (a) Local distortion to the prism that will cause the energy levels to shift.(Left/Right side) When the prism is compressed/elongated along the c-axis and ex-panded/compressed in basal plane, energy of dz2 will be lowered/increased. (b) Constantcurrent image with atomic corrugation filtered out serves as a guide for local distortion inchalcogen layer.
Similar to the Jahn-Teller effect in manganites , the subtle change in local coor-
dination will cause energy shift in the d orbitals and result in a partial orbital ordering.
The main difference between a charge ordering and an orbital ordering is that in the former
electrons shift from one lattice site to another, while in the latter they transfer from one
orbital to another on the same atom. Moreover, if the M-M bond length is also reduced
, the overlap of the dxy/dx2−y2 orbitals will be further enhanced . Both the partial
orbital ordering and the enhancement of hopping could reduce the energy of electron system
by pulling down the filled dxy/dx2−y2 band that extends deeply below EF , in accordance
with high energy electron being involved . It is a strong possibility that this orbital or-
dering will explain the enhanced conductivity as we mentioned earlier, since it can enhance
the in-plane hopping of electrons. In the topographic image (Fig. 4.5b) we can see that the
areas with enhanced in-plane hopping are connected, which is consistent with an increase of
conductivity. It will also likely change the electronic scattering rate (for part of the Fermi
surface) and result in the large Nernst signal related to CDW formation in the multi-band
system NbSe2 .
-200 -100 0 100 200VBias(mV)
Figure 4.6: 10 × 10 nm2 LDOS ratio map of TaS2 at T = 52 K. The upper part is at aregion with CDW misalignment, and the lower part shows very similar ratio structure withTaSe2.
Furthermore, we have performed similar experiments in TaS2 and the intra-unit-cell
variation of LDOS is very similar indicating that the orbital degree of freedom has a generic
effect on the formation of CDW in this class of materials.
It is indeed possible that the asymmetry is varying due to variations in the tip height,
if the filled and empty states decay into the vacuum with drastically different characteristic
lengths. However, this possibility has been ruled out by comparing the asymmetry with
another data set taken at a different setup tip height (Fig. 4.7) which shows identical results.
-100 -50 0 50 100VBias(mV)
Figure 4.7: Averaged LDOS spectra with two different setup conditions: −200 mV 300 pAand −100 mV 100 pA. The average difference in tip height is about 15 pm, while theasymmetry difference is only 1%.
In conclusion, we have shown that the common kink feature around 32 mV is not
related to CDW and suggested they can be explained by phonon-assisted inelastic tunneling.
By correlating the LDOS asymmetry with the lattice distortion, we have provided strong
evidences for a partial orbital ordering in the 2H-MX2. Such an orbital ordering, although
not as evident as the one in manganites, still has important implication on the unexpected
transport behaviors and is very likely associated with the driving mechanism of CDW in
2H-MX2. The discovery of this orbital ordering benefits from the tunneling process heavily
favors one of the orbitals, which initially seemed to be a drawback. This methodology will
be useful for future study of orbital physics in other correlated electron systems.
Local density of states study of 5d Mott insulator Sr2IrO4
5.1 Introduction to Mott physics
5.1.1 Mott insulator
Mott insulators are insulating materials due to strong electron-electron correlation
effects, which according to the conventional band theory are ought to be conductors with
partially-filled conduction band . Here, the electron-electron correlation effect usually
refers to the intra-atomic (on-site) Coulomb repulsion interaction between electrons, defined
where φ1 and φ2 are the wave functions of the two electrons under consideration and r12
is the distance between them. From Eqn. (5.1), we can see why U will be large if the two
electrons occupy orbitals that largely overlap with each other or (for most of the times) the
same orbital. Furthermore, U will also be increased if the orbital is constrained to little
space, i.e. localized, due to the decreased average distance between electrons. For instance,
3d electrons usually have much larger U than 4d and 5d electrons.
Early studies were related to explain the insulating behavior in many 3d transition
metals, like CoO, where the localized the 3d orbitals play an important role of raising the
on-site U. Relatively recent studies focused on ternary transition metal compounds like
La2CuO4 and LaMnO3, where interesting physics like unconventional superconductivity and
colossal magneto-resistivity arise when the compound is chemically doped cite .
A simple view of the Mott insulator could be established by considering an artificial
sodium crystal with N atoms, where the lattice constant a is tunable. In this model the energy
cost of double occupancy (U) is constant, but the electron kinetic energy t is increasing with
decreasing a, and hence the energy bandwidth (W ). The energy gain of forming a half-
filled band can be understood via the the process of two sodium atoms forming one Na2
molecule; the two electrons only occupy the bonding orbital and leave the anti-bonding
orbital empty and gain energy 2t. Following this reasoning, one can find that energy gain by
forming a half-filled band in the sodium crystal is 1/4NW . At the mean time, since electrons
distribute randomly between the lattice sites, a certain number of lattice sites will be doubly
occupied and will increase the system energy by 1/4NU . It could be naively concluded that
a transition occurs at,
U = W. (5.2)
When U < W , the system favors forming the band so it is metallic; when U > W , the
system favors singly occupied state so it is insulating.
Figure 5.1: Density of states change during a Mott transition. When U < W the systemis metallic and when U > W there is an energy gap between the lower and upper Hubbardbands.
5.1.2 Hubbard model
A commonly used theoretical model for describing Mott insulators is the Hubbard
H = −t∑
c†iσcjσ + c†jσciσ
where the c†iσ and cjσ are the electron creation and annihilation operators on lattice sites i
and j, 〈i, j〉 means nearest neighboring sites and niσ is the number operator on lattice site i.
This model gives the minimum description for realistic correlated systems, but is not
exactly solvable in cases like the 2d/3d square lattice. However, some qualitative picture
can be obtained by analyzing the limits of U ≫ t and U ≪ t. When U is small, the system
is simply metallic with bandwidth W = 2zt, where z is the coordination number. When
U is large, the system is insulating and energy gain via t is on the order of −t2/U , the
result of a second-order perturbation, which only happens when neighboring electron spins
are anti-parallel. This is the reason why a lot of Mott insulators are anti-ferromagnetic, as
a result of strong electron-electron correlation.
5.2 The novel Jeff=1/2 Mott insulator Sr2IrO4
5.2.1 Spatial extensions of d orbitals
The fairly localized 3d electrons have large el-el correlation, which is lowered in the
delocalized 4d and 5d electrons. The spatial extensions of d-orbitals with different principal
quantum numbers could be seen in Fig. 5.2, with their radial wave functions being,
(42− 14ρ+ ρ2)ρ2Z3/2e−ρ/2,
where ρ is the reduced radius ρ = 2Zr/na0, Z is the effective nuclear charge, and a0 = 0.53A
is the Bohr radius.
In Fig. 5.2, we have used effective charge Z = 5 for all three of them. We clearly see
how the d orbital extensions change with respect to the principal quantum number n. The
5d orbital is almost 3 times (in length) large than the 3d orbitals; with a lattice constant
of a = 4A which is reasonable most of the transition metal oxides, the 3d electrons are well
isolated from each other, while the 5d electrons will be ‘touching’ one another. It should be
noticed that the size of the orbitals are scaled by the effective nuclear charge, so it could
vary a lot between elements even with the same principal quantum number n, or even the
same element but with different oxidization states or crystal environment.
Figure 5.2: Spatial extensions of d orbitals, assuming the same effective charge numberZ = 5. Left: the radial wave function of the d orbitals, Rnd(r). Right: the probabilitydistribution p(r) = r2Rnd(r)
2. The shaded area roughly indicates the inter-atomic distances.
Following Eqn. 5.1, we can make some ‘naive’ comparison of the on-site Coulomb
repulsion energies: U3d equals to a few times of U5d. However, the exact numbers for ions in
real solids are not easy to figure out from first principle and they will vary from one element
to another even with the same principal quantum number. In reality, Hubbard-U is treated
as an adjustable parameter for calculations for the most of the time.
5.2.2 Spin-orbit coupling
Spin-orbit interaction can be understood as the result of spin alignment in the effective
magnetic field felt by the electron, while the magnetic field is introduced by Lorentz trans-
formation of the nuclear electrical field. It is one of the relativistic effects inside atoms and
can be describe by the following Hamiltonian,
H = ζnl L · s, (5.5)
where L and s are the angular momenta of orbital and spin, and,
is an integral involving the electric field strength and the radial wave function Rnl(r). The
exact form of this integral can be found in text book . As pointed out by Tinkham ,
the integral of ζnl favors the interior of the atoms, and hence the screening effect by other
valence electrons is much less than when one is trying to compute the out-most electrons’
wave functions. As a result, ζ increase rapidly with respect to Z, ζ ∼ Z4. For iridium with
Z = 77, ζ is about 0.5 eV in the atomic limit .
However, it does not necessary mean that spin-orbit coupling will always be large in
heavy elements, since more often than not the orbital angular momentum is quenched in a
solid via crystal field splitting of the nl manifolds. In the case of Sr2IrO4, the t2g manifold
with dxy, dyz and dzx orbitals serves with an effective angular momentum leff = 1. It is the
coupling of this effective angular momentum with the spin that causes the interesting physics
we are talking here in this chapter.
5.2.3 Spin-orbit Mott insulators
As we mentioned above, the correlation effect (U) decreases in the d orbitals when
the principal quantum number n increases. It is for this reason that most 4d transition
metal oxides are good metals (e.g. Sr2RuO4 and Sr2RhO4), unlike their 3d cousins (e.g.
La2CuO4, LaMnO3). Iridium oxides like Sr2IrO4 and Na2IrO3, with 5d electrons, were
expected to be more metallic than the 4d transition metal oxides. However, many iridium
oxides, including the two we mentioned, are insulators [83, 84, 85, 86]. B. J. Kim et al.
proposed the SOC-induced Mott insulating idea after studying Sr2IrO4 with angle-resolved
photoemission spectroscopy (ARPES), optical conductivity and various other methods .
In this picture, the t2g manifold is further split by SOC into two multiplets, a Jeff = 1/2
doublet and a Jeff =1/2 quartet, with the atomic limit separation between them being 32ζ.
With the 5d5 electron configuration, the quartet band with lower energy is fully occupied
and the doublet band become half-filled with a much smaller bandwidth (W). In this limit,
a small electron correlation will cause the system to undergo Mott transition band become
an insulator, as illustrated in Fig. 5.3. It is then very similar to the square lattice Hubbard
model with exactly half-filling of the band.
atomic octahedral tetragonal spin-orbit
Sr O Ir
Figure 5.3: Splitting of 5d levels in Sr2IrO4. The tetragonal splitting of the t2g manifold is∆ ≤ 100meV and the SOC splitting is on the order of ζ = 0.5 eV. When the SOC dominates,the electron spin is no longer a good quantum number and the Jeff states are mixtures ofspin states. Inset: the local environment of the Ir4+ ion.
After the discovery of this Mott insulator, physicists quickly realized that Sr2IrO4 is a
very close analogy to La2CuO4, the parent compound of high-Tc superconductor . This
leads to the proposals like achieving superconductivity in this material via chemical doping
[88, 89]. More interestingly, this material, together with the 213 compounds, are possible
testbeds for exotic spin models like the quantum compass and Kitaev models [90, 91, 92].
However, one of the similarities to La2CuO4, which relies on Sr2IrO4 being in the strong
SOC limit so that only the Jeff = 1/2 band need be considered, becomes less certain when
one realizes that the electron hopping energy (t ≈ 0.3 eV [88, 89]) is close to the SOC
energy (ζ ∼ 0.5 eV ). Furthermore, instead of the Mott-type insulator, the magnetically
originated Slater insulator has also been proposed , supported by time-resolved optical
A key to identify the nature of this insulator is to answer the important questions of
what is the size of the insulating gap, ∆, and how does it compare to other energy scales (e.g.
t and ζ). Surprisingly, measurements of gap size from different probes in Sr2IrO4 vary widely.
Gaps of ∼ 0.1 eV have been reported by fittings of the resistivity data with the thermal
activation model [95, 96] and by calculations using local density approximation (LDA) with
SOC and U [74, 97]. On the other hand, angle-resolved photoemission spectroscopy (ARPES)
measurements do not agree with this value since the maximum of the valance band is already
lower than −0.1 eV [74, 98]. Optical conductivity and resonant inelastic x-ray scattering
(RIXS) studies both yield ∆ ≤ 0.4 eV [87, 99]. Importantly, these measurements are (either)
indirect, susceptible to signals from other excitations like exciton or magnon, and/or can only
measure the filled states, making the interpretations of their gap values difficult. It is highly
desirable to measure the gap with an experiment that directly probes the free charge carriers.
5.3 Study of insulating gap in Sr2IrO4 with STS
STS is a direct probe for the electronic density of states and hence the insulating gap (if
any) of a material, since it utilizes the single particle tunneling effect and is free of excitonic
effect or magnetic excitation. Measurements of insulating gaps have been demonstrated in
various places [100, 101]. We have performed STM and STS experiments on Sr2IrO4 at the
temperature of 80 K with our UHV-STM system.
Sr2IrO4 has the K2NiF4-structure and can be cleaved between the two adjacent and
identical SrO layers. Fig. 5.4a shows a 20 × 20 nm2 constant-current image taken with
−300 mV and 5 pA, in which we can see the Sr square lattice in the top layer (Fig. 5.4b).
The Fourier transform (Fig. 5.4c) of this topographic image shows four strong atomic peaks,
confirming the high quality of this surface. The oxygen atoms do not appear in topography
likely due to the tunneling voltage being far away from the O 2p levels at −3.3 eV .
Together with the atomic lattice, the sample also shows a small number of defects with the
most evident type being the dark patches (see below).
(b) Sr O Ir
Figure 5.4: Topography and atomic structure. A 20×20 nm2 topographic image taken with−300 mV and 5 pA at 80 K (a) and its Fourier transform (c). The black arrows indicatethe a and b axes of the crystal lattice. Red and blue arrows indicate two Sr-related defects.(b) Schematic diagram of the first SrO and second IrO2 layers of a cleaved surface. Thesquare lattice in (a) correspond to Sr in top layer. The image has been processed to removevibrational noise at a certain frequency.
Shown in Fig. 5.5a is a LDOS spectrum measured by averaging ∼1300 spectra taken
over a 2×2 nm2 area that did not include any apparent defects. The negative sample-bias
side of the LDOS, corresponding to the occupied states, shows no distinct feature that can
be related to the lower Hubbard band (LHB) of Jeff=1/2 band down to −1 eV (Fig. 5.5b),
contrasting to the double-peak structure observed in optical conductivity measurement .
However, optical measurements in insulators are sensitive to excitons  and Kim et al.
 have pointed out that the double-peak seen in the optical conductivity cannot be due
to the Jeff = 3/2 (quartet) and LHB of Jeff = 1/2 bands. In Na2IrO3 and Li2IrO3, the
importance of excitonic effect has been shown by a recent RIXS study . It is therefore
strongly possible that the LHB of Jeff =1/2 band is overlapping with rather than separate
from the quartet band, in good agreement with calculations done by LDA+DMFT  and
variational cluster approximation . According to Watanabe et al. , the LHB is entirely
enclosed by the quartet band. This overlap between LHB and quartet bands implies that
the strong SOC limit and single band models are inadequate for Sr2IrO4 and many-body
effect should be taken into account.
The insulating gap from our tunneling spectra is about 620 meV, with the valence
band top at −150 meV and conduction band bottom at +470 meV (Fig. 5.5a). Here the
energy gap is defined as the size of the energy window with no coherent density of states.
The energy of the valence band top (−150 meV) is in excellent agreement with the one
measured by ARPES [74, 98]. The slow rise in the LDOS between 0.2 and 0.5 eV varies with
tunneling location and hence we believe it is extrinsic either due to local impurity states
or varying tip-induced band bending. LDOS measurements on a set of points which are all
far away from any defects show that the slow rise only appears in some (Fig. 5.5c) but not
the rest of the spectra (Fig. 5.5b). On the other hand, the gap edges at −150 and +470
meV are independent of location. Therefore, the large 620 meV gap is due to the underlying
nonlocal, energy bands and the inhomogeneous in-gap states are caused by the local defects.
Furthermore, LDOS measurements in Rh-doped sample Sr2Ir1-xRhxO4 (x = 0.04)  also
confirm this by showing that far from the intentional impurities a similarly sized large gap
However, this large gap is not in good agreement with the gap values reported so far.
In the similar material La2CuO4, the debate about the gap size has been lasting for long
time [107, 108, 109] because of preciously similar subtleties. The difficulty in extracting the
correct energy scale of the intrinsic gap rises when other processes are involved, as stated
above. STS, on the other hand, can measure the Mott gap directly through the single-
particle tunneling process. It does require a tunneling current going through the sample and
may have difficulty for materials with poor electrical conductivity, but we have overcome
-0.8 -0.6 -0.4 -0.2 0 0.2 0.4 0.6VBias(V)
-1.0 -0.5 0.0 0.5VBias(V)
(d) Jeff =3/2 LHB UHB
Figure 5.5: The large intrinsic energy gap. (a) LDOS measured by averaging 36×36 spectraover the 2×2 nm2 area indicated by the black square in the topographic image (inset). Thedashed lines are drawn to indicate the band edges at −150 mV and +470 mV. Data wastaken with -300 mV and 10 pA and ac modulation of 8 mVrms at 2.2 kHz. (b) and (c) LDOStaken at different ‘intrinsic’ locations away from the defects, (b) without and (c) with theslow rise. (d) Diagram showing energy bands with two important features: the 620 meVinsulating gap and the overlap between the LHB and the Jeff=3/2 bands.
this problem by performing the experiment at liquid nitrogen temperatures and with very
low tunneling currents, minimizing the tips’ electric fields.
This 620 meV gap strongly implies that Sr2IrO4 is a relatively weak Mott rather than
Slater insulator, since the magnetic coupling energy is merely 60−100 meV [87, 110], too
small to account for the large gap. Additionally, this is also consistent with the transport
measurement showing no insulator-to-metal transition at least up to 600 K . Although
the size of this gap is considerably smaller than the 3d cuprates [101, 107], it is still large
compared to what one would expect from the extended 5d orbitals and the fact that Sr2RhO4
is actually a paramagnetic fermi liquid [112, 113]. The band minimum of the upper Hubbard
band (UHB) of the Jeff = 1/2 band, is the major discrepancy between our STS result and
the existing studies. LDOS measurements show that the band minimum of UHB is at +470
meV, implying that LDA calculation needs a larger Hubbard-U to capture this feature since
it has been shown that the insulating gap depends on U sensitively . In a recent study
on Na2IrO3, Comin et al.  have shown that using U as large as 3 eV in LDA calculation
is necessary to reproduce the 340 meV gap in that material. With this work a stronger
than expected correlation effect has now been observed in two iridates. The measured gap
in Sr2IrO4 is nearly twice the measured gap seen in Na2IrO3, indicating that in the material
studied here the 5d electrons are even more correlated (larger U/W).
The spatially extended nature of the 5d electrons can indeed largely reduce the on-site
Coulomb repulsion, but at the meantime will increase the same type of interaction between
the electrons sitting on neighboring Ir sites due to the increased overlap of their wave func-
tions. The neighboring Coulomb interaction had been theoretically studied in the extended
Hubbard model . For Sr2IrO4, the Wannier functions calculated by Jin et al.  do
show that a significant amount of electron weight is distributed on the four neighboring sites.
It is thus strongly possible that the symmetric arrangement of the neighbors can result in
a net repulsion that appears to be on-site. Interestingly, Ir4+ in Sr2IrO4 has four nearest
neighbors while it has only three in Na2IrO3, in agreement with their gap sizes, if the neigh-
-0.3 -0.2 -0.1 0 0.1 0.2 0.3VBias(V)
Dark spot, -300mV/100pA
Figure 5.6: (a-d) Images of defects with a wide range of junction resistances: 3.3−100 GΩ.The + signs indicate defects looking differently with different tunneling conditions. (e) LDOSmeasured on a dark spot (defined as the red cross in (a)). These images have been processedto remove vibrational noise at a certain frequency.
boring interaction is indeed causing a larger Hubbard-U. Moreover, Ba2IrO4, another iridate
insulator  with a larger bandwidth W by not having the octahedra rotation, further
confirms the strong entanglement of the energy scales in the 5d electrons.
5.4 Large insulating gap measured in Sr2Ir0.96Rh0.04O4
We have also measured a similarly sized gap in some area of a Rh-doped sample
Sr2Ir0.96Rh0.04O4 (Rh4). In Fig. 5.7 we have shown a topographic image of the Rh4 sample
and a gap map for the same area. The image in (a) was taken at -800 mV (20 pA), while
the gap size in (b) was defined by energy locations where the measured dI/dV spectra pass
a threshold value (0.05 in the this case). In Fig. 5.7c, we see a dI/dV curve measured by
averaging the measurements on areas defined by green circles/ellipses in (a). This dI/dV
clearly shows that the large gap survives at some areas of the Rh4 sample when they are far
away from the dopants.
5.5 Study of impurity effects on insulating gap
To understand the effects caused by the defects, we have further studied topography
at different junction resistances and LDOS on and off the defects. We see two types of Sr-
related defects in the topography: Sr vacancy (the faint feature indicated by the red arrow in
Fig. 5.4a) and Sr ad-atom (the bump in between four Sr atoms indicated by the blue arrow
in Fig. 5.4a). These two types of defects could be caused by the cleaving process, but have
little effects on the local electronic structure. In stark contrast the third type of defect we
see, the dark patches, has a large effect on the local electronic structure. We identify these
dark-patch defects in Sr2IrO4 as being excess/deficiency oxygen atoms, similar to those seen
in manganite  and cuprate [117, 118]. This is in accord with the fact that Sr2IrO4 can
have various levels of oxygen deficiency [119, 120], but more work is needed for a definitive
Topographic images (Fig. 5.6) with junction resistance ranging from 3.3 to 100 GΩ
Figure 5.7: Large insulating gap measured on Sr2Ir0.96Rh0.04O4. (a) A 36 × 36 nm2 topo-graphic image of Rh-doped Sr2IrO4, (b) Map of gap size measured on the same area as (a)with the red squares indicating the locations of Rh dopants. The gap here is defined thepoints where dI/dV spectra crosses a threshold value. (c) A representative dI/dV curve thatlooks similar to that measured on the parent compound.
confirm that the patchiness originates from defects that are related to electronic inhomo-
geneity other than structure corrugation. The cross signs in Fig. 5.6a-d indicate the areas
that look differently with different tip-sample separations. Such a high sensitivity in topog-
raphy with respect to the tunneling condition reflects the fragile insulating nature of Sr2IrO4
in the presence of perturbation, and also the potential influence to the sample brought by
O defects. Additionally, it is known that for some transition metal oxides, oxygen atoms in
surface layers are volatile, but we didn’t observe any degradation of surface quality in several
days at 80 K implying the stability of the surface. Therefore, these O related defects are
likely intrinsic to the sample, in accord with O deficiency found in the system [119, 120]. This
result naturally explains why transport measurements give a smaller gap [95, 96] and optical
conductance shows a slow rise starting at 0.2 eV . The presence of these defects leads to
in-gap states, lowers the effective gap measured by transport and gives a lower energy scale
for optical transitions. More importantly, the random distribution of the defects is in good
agreement with the variable-range-hopping behavior in electrical conductivity . The ex-
istence of intrinsic defects despite the good sample quality and our ability of measuring the
intrinsic LDOS apart from the influence of defects, prove the necessity of using a local probe
like STM to study this material.
Lastly, the LDOS study on top of a defect (Fig. 5.6e) shows how strongly it can change
the density of states around EF by building up in-gap states. It should be admitted that,
due to the dramatic difference in topography of this defect as we mentioned earlier, the
STS measurement may not be reflecting the underlying LDOS accurately, but it should be
sufficient to serve as evidence for the in-gap states. Fig. 5.8 shows the subtle variation in
the measured spectra related to the tip-induced band bending, calling out the necessity of
measuring with high junction resistances.
-0.3 -0.2 -0.1 0.0 0.1 0.2 0.3VBias(V)
Figure 5.8: LDOS measured at a normal lattice site with different junction resistances: 10GΩ (purple) and 1 GΩ (green). The difference could be accounted by tip-induced bandbending. Inset: topographic image with the cross sign defining the spot of data taking.
As a summary, we have presented the first atomic-scale study in Sr2IrO4 with density
of states measurement covering the entire Mott gap, which is 620 meV. The measurement of
the occupied states has confirmed the overlap between LHB and quartet band. We concluded
that Sr2IrO4 is a Mott but not Slater insulator by comparing the gap size with the magnetic
coupling energy, implying the stronger-than-expected el-el correlation in this 5d system.
Furthermore, we suggested that additional source of Coulomb repulsion need to be taken
into account to quantitatively understand the 5d electron systems. Lastly, the junction
dependence of the defects in the topography, together with the LDOS results about the
defects, indicate their profound impacts on the local electronic structure of a 5d system.
Our results strongly imply that in Sr2IrO4 the three energy scales (SOC, U and W) are
strongly competing against each other and that studying the 5d electrons should put all of
them on equal-footing.
Vibration test of Room E2B37
We have measured the background vibration of the room E2B37 with a geophone. Since
the geophone is only sensitive to noise above 1 Hz, the measurements here were subjected
to this low frequency cut-off. The voltage signals coming out of the geophone were then
connected to a Fourier spectrum analyzer (SR760).
0 50 100 150 200
Horizontal vibration on the floor
Horizontal vibration on the pad
0 50 100 150 200
Figure A.1: Vibrational test of Room E2B37 measured by the geophone SN-1211 (Geo SpaceCorporation).
The tests have been done with several different conditions: normal is with people
working inside the room; quiet is with all of the electronics turned off and only the test person
staying inside; noisy outside is with people jumping in the hallway out of the room; and noisy
inside is with people jumping inside the room. Furthermore, prior to the construction of our
STM lab, there was a concrete pad on the floor that was isolated from the rest of the floor.
The pad was about 3 by 5 feet in area and 3 feet in depth into the ground. This pad was
also tested for vibration. The test results of all of the above conditions were summarized in
Fig. A.1. One major noise component in this room is at 30 Hz. As we can see the difference
between ‘floor’ and ‘pad’ is mainly the overall shape of the vibrational noise: the pad tended
to suppress high frequency vibration but enhance low frequency components (less than 60
Hz). Because STM experiment is very sensitive to noise from DC to a few hundred Hz, we
decided that we won’t be able to benefit from the pad. It is also clear that noise on the
hallway outside the room E2B37 is not increasing the vibration inside very much. Only when
the noise is originated inside the room, there is a large enhancement of the vibration at high
Pressure vs. time in a UHV pumpdown
In order to achieve ultra-high vacuum (UHV), we firstly need to pay attention to the
materials that are used inside the vacuum chamber as we discussed in Ch. 1. An important
criteria for choosing the materials is that they need to be sustainable with high temperature
bake-out (at least up to 150 C) without increased outgassing, chemical decomposition or
losing mechanical strength. The bake-out process is crucial for achieving UHV environment;
without a bake-out the UHV-STM system is only able to achieve ∼ 10−9 torr, but with a
bake-out the base pressure is decreased by a factor of 10. With the further pressure reduction
by cooling down the two dewars, the ultimate pressure of the system is about 5× 10−11 torr.
Shown in Fig. B.1 is a plot of pressure versus time for a normal bake-out process.
The turbo pump is turned on at the beginning, with the ion pump and the bake-out heating
turned on the next day. Here turning on the ion pump means opening the gate valve between
the chamber and the ion pump, while the ion pump itself was powered on all the time and
pressure sitting below 10−10 torr. For the first day the entire chamber is only pumped via
the turbo pump connected to the load-lock with the pressure ended up with low 10−6 torr
range. When the ion pump is turned on (opening of the gate valve between the ion pump
and the STM chamber), the pressure dropped to 2× 10−7 torr immediately.
The next step is to turn on the heat for the bake-out, which results in the slow rising
of chamber pressure back to 10−6 torr during the following few hours, with the ultimate
pressure of the bake-out being ∼ 10−7 torr. During the bake-out the chamber pressure
Figure B.1: Plot of pressure versus time of the UHV-STM system during a bake-out process.The turbo pump was turned on at the beginning, while the ion pump and the bake-out heatwere turned on at the second day. The pressure spikes were due to TSP flashes, which weremade more frequent towards the end of the bake-out. The barely visible down-turn of thepressure at the very end of the curve is due to the termination of the bake-out heating, whichresulted in a pressure decrease to low 10−9 torr within a day. Further pumping, togetherwith TSP flashes, reduced the chamber pressure to 2× 10−10 torr prior to the cooling downwith LN2.
decreased slowing to low 10−7 torr range in several days, which is mainly limited by the turbo
pump speed and the low pumping conductance via the load-lock. If there were an additional
turbo pump that is attached the chamber itself, this process will be largely shortened. In
the process of the bake-out, the chamber temperature were raised to ∼ 120 − 140 C in a
few hours but the STM scan-head temperature increased to ∼ 120 C in about 2 to 3 days.
Further bake-out after this point won’t help reducing the pressure by much.
During the bake-out shown here in Fig. B.1, the pressure was further decreased using
more frequent TSP flashes. During the normal operation when there is no heat on the
chamber, one TSP flash is usually with 48 A current through the TSP filament for 1 to 2
minutes, with the frequency being once per day or even less. However, during a bake-out,
the TSP cartridge inside the ion pump is already at temperature of 200 C without any
current, so current of 48 A will burn the TSP filament very quickly. Instead of 48 A, we
have used current like 35 A which is sufficient for baking the filament itself. If we need to
utilize the pumping power of the TSP, we usually use current of ∼ 43 A.
Figure B.2: .Plot of pressure versus time of the UHV-STM system during normal operation.
A pressure versus time chart is shown in Fig. B.2. We can see that the base pressure
during this period of time is about 7 × 10−10 torr instead of 5 × 10−10 torr, since only LN2
were used and the STM temperature was set to 80 K. When the turbo pump is turned
on for pumping the load-lock, the chamber pressure will increase slowly to 1 × 10−10 torr.
This slow rise of pressure is probably associated with the mechanical vibration of the turbo
pump which can expedite the outgassing of gas molecules off the chamber. Every time when
the gate valve between the load-lock and the chamber was opened for sample manipulation,
there was a pressure spike (2− 5× 10−10 torr) even though the load-lock had been pumped
for hours. The last part of that curve was showing the process of the outer dewar warming
up due to outage of LN2. This happens if the LN2 is not refilled within 72 hours from the
We have done a transient response study of the STM feedback system, following Ref. .
A simplified diagram of the feedback system is shown in Fig. C.1. Signals in this feedback
loop are all voltages except the tunneling current prior to the amplification.
Figure C.1: Feedback loop for the constant current imaging mode. The pre-amp convertstunneling current into voltage signal. The ‘log’, ‘comparison’ and ‘times gain’ operations areall done by the STM controller.
In this feedback loop, the tunneling current I = I0e−(zs−zt)/κ is amplified by the pre-
amp, V = I × Rf . The log of this signal is then compared with the set value, and the
resultant error is then sent to the gain plant to produce the voltage signal that drives the z
piezo (moves the tip back and forth). The gain of the loop is then defined by the following
G = 2κ ·KV ·Kz ·KI (C.1)
where κ = 10 nm−1 (1 A−1), KV = log10 e = 0.4343, Kz = 2.4 nm/V and KI is the integral
gain from user input.
The transfer functions of the system are as follows,
T1(s) = 1 + t1s+1
(1 + t3s)
T2(s) = 1 + t2s+1
(1 + t2s)
R(s) =G(1 +Kps)
G(1 +Kps) + s× T1(s)× T2(s)×(
1 + s2
where T1(s) and T2(s) are the transfer function of the two stages in the current pre-amplifier
and R(s) is the total transfer function of this feedback loop. Using R(s) we can do a
transient response analysis by forward and inverse Laplace transformations for a set of given
0.998 1.000 1.002 1.004 1.006 1.008 1.010
Figure C.2: Transient response of the tip when scanning through a height step. The bluecurve is the ideal response or the actual surface topography. The purple/red curves indicatesituations with proper or unstable gain settings. This simulation was done by forward andinverse Laplace transformation in Mathematica.
In our case, both stages of the pre-amplifiers have some significant phase shift in the
range of DC−10 kHz. In this simulation (Fig. C.2), we have used t1 = 50 µsec, t2 = 43 µsec
and t3 = 0.2 sec (due to shunt capacitance Cs = 200 pF and feedback resistor Rf = 1 GΩ).
We have chosen Q = 1000 and w = 30 kHz for our PZT8 scantube (L = 0.25, OD = 0.125,
and ID = 0.080 inch).
Another important fact is that lowering the value for w can make the system unstable
pretty quickly. The resonant frequency of the scantube decrease quickly as its length when
other parameters are fixed. The lowest resonant frequency of a tubular structured object is
mt + 0.24mc
where k = 3EIl3, I = π
64(d4o − d4i ), mt is the weight attached to the tube (In our case, the
weight of the tip assembly.) and mc is the weight of the tube itself mc = ρAl. l is the length
of the tube, E is the Young’s modulus of PZT8, A is the cross sectional area, and do/di is
the outer/inner diameters of the scantube. If there were no attached weight, mt = 0, the
relation between f and l could be further simplified as follows,
f ∼ 1
Therefore, the length of the scantube is of critical importance in determining the stability of
the STM feedback loop. Increasing the length will reduced the resonance frequency quickly
as seen in Eqn. (C.4), although it is helpful in terms of increasing the full scan size of the
STM (Eqn. (1.10)).
 L. Esaki. New Phenomenon in Narrow Germanium p-n Junctions. Phys. Rev.,109(2):603–604, January 1958.
 I. Giaever. Energy Gap in Superconductors Measured by Electron Tunneling. Phys.Rev. Lett., 5(4):147–148, August 1960.
 B.D. Josephson. Supercurrents through barriers. Adv. Phys., 14(56):419–451, October1965.
 G. Gamow. Zur Quantentheorie des Atomkernes. Zeitschrift fur Physik, 51(3-4):204–212, March 1928.
 C.J. Chen. Introduction to scanning tunneling microscopy. Oxford University Press,USA, 1993.
 J. Bardeen. Tunnelling from a Many-Particle Point of View. Phys. Rev. Lett., 6(2):57–59, January 1961.
 G. Binnig, H. Rohrer, Ch. Gerber, and E. Weibel. Surface Studies by Scanning Tun-neling Microscopy. Phys. Rev. Lett., 49(1):57–61, July 1982.
 S.H. Pan, E.W. Hudson, and J.C. Davis. 3He refrigerator based very low temperaturescanning tunneling microscope. Rev. Sci. Instrum., 70(2):1459, February 1999.
 K. Besocke. An easily operable scanning tunneling microscope. Surface Science, 181(1-2):145–153, March 1987.
 G. Binnig and D.P.E. Smith. Single-tube three-dimensional scanner for scanning tun-neling microscopy. Rev. Sci. Instrum., 57(8):1688, August 1986.
 D. Coyne et al.. LIGO vacuum compatible materials list. LIGOE960050-BE (LaserInterferometer Gravitational Wave Observatory, 2004), 2004.
 G. Gruner. Density waves in solids. Addison-Wesley Reading, MA, 1994.
 H. Yeom, S. Takeda, E. Rotenberg, I. Matsuda, K. Horikoshi, J. Schaefer, C. Lee,S. Kevan, T. Ohta, T. Nagao, and S. Hasegawa. Instability and Charge Density Waveof Metallic Quantum Chains on a Silicon Surface. Phys. Rev. Lett., 82(24):4898–4901,June 1999.
 E. DiMasi, M. Aronson, J. Mansfield, B. Foran, and S. Lee. Chemical pressure andcharge-density waves in rare-earth tritellurides. Physical Review B, 52(20):14516–14525, November 1995.
 A. Fang, N. Ru, I. Fisher, and a. Kapitulnik. STM Studies of TbTe3: Evidence for aFully Incommensurate Charge Density Wave. Phys. Rev. Lett., 99(4):6–9, July 2007.
 G. Gruner. The dynamics of charge-density waves. Rev. Mod. Phys., 60(4):1129, 1988.
 P. Monceau. Electronic crystals: an experimental overview. Adv. Phys., 61(4):325–581,August 2012.
 K. Rossnagel. On the origin of charge-density waves in select layered transition-metaldichalcogenides. J. Phys.: Condens. Matter, 23(21):213001, June 2011.
 D. S. Dessau, Z.-X. Shen, D. M. King, D. S. Marshall, L. W. Lombardo, P. H. Dick-inson, A. G. Loeser, J. DiCarlo, C.-H Park, A. Kapitulnik, and W. E. Spicer. Keyfeatures in the measured band structure of Bi2Sr2CaCu2O8+δ: Flat bands at EF andFermi surface nesting. Phys. Rev. Lett., 71(17):2781–2784, October 1993.
 K. Terashima, Y. Sekiba, J. H Bowen, K. Nakayama, T. Kawahara, T. Sato, P. Richard,Y-M Xu, L J Li, G H Cao, Z-A Xu, H Ding, and T Takahashi. Fermi surface nestinginduced strong pairing in iron-based superconductors. Proc. Natl. Acad. Sci. USA,106(18):7330–3, May 2009.
 W.D. Wise, M.C. Boyer, K. Chatterjee, T. Kondo, T. Takeuchi, H. Ikuta, Y.Y. Wang,and E.W. Hudson. Charge-density-wave origin of cuprate checkerboard visualized byscanning tunnelling microscopy. Nature Phys., 4(9):696–699, July 2008.
 C. Brun, Z.Z. Wang, and P. Monceau. Scanning tunneling microscopy at the NbSe3surface: Evidence for interaction between q1 and q2 charge density waves in the pinnedregime. Phys. Rev. B, 80(4):045423, July 2009.
 J. Carpinelli, H. Weitering, E. Plummer, and R. Stumpf. Direct observation of asurface charge density wave. Nature (London), 381(6581):398–400, May 1996.
 J. Carpinelli, H. Weitering, M. Bartkowiak, R. Stumpf, and E. Plummer. SurfaceCharge Ordering Transition: α Phase of Sn/Ge(111). Phys. Rev. Lett., 79(15):2859–2862, October 1997.
 K. Rahnejat, C. Howard, N. Shuttleworth, S. Schofield, K. Iwaya, C. Hirjibehedin,Ch. Renner, G. Aeppli, and M. Ellerby. Charge density waves in the graphene sheetsof the superconductor CaC6. Nat. Commun., 2:558, January 2011.
 J.A. Wilson and A.D. Yoffe. The transition metal dichalcogenides discussion andinterpretation of the observed optical, electrical and structural properties. Adv. Phys.,18(73):193–335, May 1969.
 B. Sipos, A. Kusmartseva, A. Akrap, H. Berger, L. Forro, and E. Tutis. From Mottstate to superconductivity in 1T-TaS2. Nature Mater., 7(12):960, December 2008.
 T. Hanaguri, C. Lupien, Y. Kohsaka, D.H. Lee, M. Azuma, M. Takano, H. Tak-agi, and J. Davis. A ‘checkerboard’ electronic crystal state in lightly hole-dopedCa2−xNaxCuO2Cl2. Nature, 430(7003):1001–5, August 2004.
 S. Slough, W. McNairy, and R. Coleman. Charge-density waves studied with the useof a scanning tunneling microscope. Phys. Rev. B, 34(2):994, 1986.
 R. Coleman, B. Giambattista, P. K. Hansma, A. Johnson, W. McNairy, and C. Slough.Scanning tunnelling microscopy of charge-density waves in transition metal chalco-genides. Adv. Phys., 37(6):559–644, December 1988.
 H. Hess, R. Robinson, R. Dynes, J. Valles, and J. Waszczak. Scanning-Tunneling-Microscope Observation of the Abrikosov Flux Lattice and the Density of States nearand inside a Fluxoid. Phys. Rev. Lett., 62(2):214, October 1989.
 X.L. Wu and C. Lieber. Hexagonal Domain-Like Charge Density Wave Phase of TaS2
Determined by Scanning Tunneling Microscopy. Science, 243(4899):1703–5, March1989.
 C. Wang, S. Slough, and R. Coleman. Spectroscopy of dichalcogenides and trichalco-genides using scanning tunneling microscopy. J. Vac. Sci. Technol. B, 9(2):1048, March1991.
 H. Hess, R. Robinson, and J. Waszczak. STM spectroscopy of vortex cores and theflux lattice. Physica B, 169:422, February 1991.
 R. Craven and S. Meyer. Specific heat and resistivity near the charge-density-wavephase transitions in 2H-TaSe2 and 2H-TaS2. Phys. Rev. B, 16(10):4583, 1977.
 Ph. Leininger, D. Chernyshov, A. Bosak, H. Berger, and D. Inosov. Competingcharge density waves and temperature-dependent nesting in 2H-TaSe2. Phys. Rev.B, 83(23):233101, January 2011.
 D. Moncton, J. Axe, and F. DiSalvo. Study of Superlattice Formation in 2H-NbSe2and 2H-TaSe2 by Neutron Scattering. Phys. Rev. Lett., 34(12):734–737, March 1975.
 G. Scholz, O. Singh, R. Frindt, and A. Curzon. Charge density wave commensurabilityin 2H-TaS2 and AgxTaS2. Solid State Commun., 44(10):1455–1459, December 1982.
 D. Moncton, J. Axe, and F. DiSalvo. Neutron scattering study of the charge-densitywave transitions in 2H-TaSe2 and 2H-NbSe2. Phys. Rev. B, 16(2):801, 1977.
 S. Borisenko, A. Kordyuk, A. Yaresko, V. Zabolotnyy, D. Inosov, R. Schuster,B. Buchner, R. Weber, R. Follath, L. Patthey, and H. Berger. Pseudogap and ChargeDensity Waves in Two Dimensions. Phys. Rev. Lett., 100(19):196402, May 2008.
 S.K. Chan and V. Heine. Spin density wave and soft phonon mode from nesting Fermisurfaces. J. Phys. F: Metal Phys., 3(4):795, 1973.
 M. Johannes, I. Mazin, and C. Howells. Fermi-surface nesting and the origin of thecharge-density wave in NbSe2. Phys. Rev. B, 73(20):205102, May 2006.
 M. Johannes and I. Mazin. Fermi surface nesting and the origin of charge densitywaves in metals. Phys. Rev. B, 77(16):165135, April 2008.
 F. Weber, S. Rosenkranz, J.-P. Castellan, R. Osborn, R. Hott, R. Heid, K.-P. Bohnen,T. Egami, A. H. Said, and D. Reznik. Extended Phonon Collapse and the Origin ofthe Charge-Density Wave in 2H-NbSe2. Phys. Rev. Lett., 107(10):107403, September2011.
 K. Iwaya, T. Hanaguri, A. Koizumi, K. Takaki, A. Maeda, and K. Kitazawa. Electronicstate of NbSe2 investigated by STM/STS. Physica B, 329-333(null):1598–1599, May2003.
 L.J. Li, Y.P. Sun, X.D. Zhu, B.S. Wang, X.B. Zhu, Z.R. Yang, and W.H. Song. Growthand superconductivity of 2H-Ni0.02TaSe2 single crystals. Solid State Commun., 150(45-46):2248–2252, December 2010.
 A. LeBlanc and A. Nader. Resistivity anisotropy and charge density wave in 2H-NbSe2and 2H-TaSe2. Solid State Communications, 150(29-30):1346–1349, August 2010.
 V. Vescoli, L. Degiorgi, H. Berger, and L. Forro. Dynamics of Correlated Two-Dimensional Materials: The 2H-TaSe2 Case. Phys. Rev. Lett., 81(2):453–456, July1998.
 R. Bel, K. Behnia, and H. Berger. Ambipolar Nernst Effect in NbSe2. Phys. Rev.Lett., 91(6):066602, August 2003.
 S. Borisenko, A. Kordyuk, V. Zabolotnyy, D. Inosov, D. Evtushinsky, B. Buchner,A. Yaresko, A. Varykhalov, R. Follath, W. Eberhardt, L. Patthey, and H. Berger. TwoEnergy Gaps and Fermi-Surface Arcs in NbSe2. Phys. Rev. Lett., 102(16):166402,April 2009.
 A. Soumyanarayanan, M.M. Yee, Y. He, J. van Wezel, D. Rahn, K. Rossnagel,E.W. Hudson, M.R. Norman, and J.E. Hoffman. Quantum phase transition fromtriangular to stripe charge order in NbSe2. Proc. Natl. Acad. Sci. USA, 1211387110,January 2013.
 D. Rahn, S. Hellmann, M. Kallane, C. Sohrt, T. K. Kim, L. Kipp, and K. Rossnagel.Gaps and kinks in the electronic structure of the superconductor 2H-NbSe2 from angle-resolved photoemission at 1 K. Physical Review B, 85(22):224532, June 2012.
 J. Demsar, L. Forro, H. Berger, and D. Mihailovic. Femtosecond snapshots of gap-forming charge-density-wave correlations in quasi-two-dimensional dichalcogenides 1T-TaS2 and 2H-TaSe2. Physical Review B, 66(4):041101, June 2002.
 E. Morosan, H. Zandbergen, B. Dennis, J. Bos, Y. Onose, T. Klimczuk, A. Ramirez,N.P. Ong, and R.J. Cava. Superconductivity in CuxTiSe2. Nature Phys., 2(8):544–550,July 2006.
 K. Wagner, E. Morosan, Y. Hor, J. Tao, Y. Zhu, T. Sanders, T. McQueen, H. Zand-bergen, A. Williams, D. West, and R. Cava. Tuning the charge density wave andsuperconductivity in CuxTaS2. Phys. Rev. B, 78(10):104520, September 2008.
 R.H. Friend and A.D. Yoffe. Electronic properties of intercalation complexes of thetransition metal dichalcogenides. Advances in Physics, 36(1):1–94, January 1987.
 S. Hufner, M.A. Hossain, A. Damascelli, and G.A. Sawatzky. Two gaps make a high-temperature superconductor? Reports on Progress in Physics, 71(6):62501, 2008.
 L.J. Li, X.D. Zhu, Y.P. Sun, H.C. Lei, B.S. Wang, S.B. Zhang, X.B. Zhu, Z.R. Yang,and W.H. Song. Superconductivity of Ni-doping 2H-TaS2. Physica C, 470(5-6):313–317, March 2010.
 R.E. Peierls. Quantum Theory of Solids. Oxford University Press, 1955.
 X.D. Zhu, Y.P. Sun, X. Luo, B. Wang, G. Li, Z. Yang, W. Song, and J. Dai. Singlecrystal growth and characterizations of Cu0.03TaS2 superconductors. J. Cryst. Growth,311(1):218–221, December 2008.
 T.M. Rice and G.K. Scott. New Mechanism for a Charge-Density-Wave Instability.Phys. Rev. Lett., 35(2):120–123, July 1975.
 A.H. Castro Neto. Charge Density Wave, Superconductivity, and Anomalous MetallicBehavior in 2D Transition Metal Dichalcogenides. Phys. Rev. Lett., 86(19):4382–4385,May 2001.
 K. Rossnagel and N. Smith. Spin-orbit splitting, Fermi surface topology, and charge-density-wave gapping in 2H-TaSe2. Phys. Rev. B, 76(7):073102, August 2007.
 C.D. Malliakas and M.G. Kanatzidis. Nb-Nb Interactions Define the Charge DensityWave Structure of 2H-NbSe2. J. Am. Chem. Soc., 135(5):1719–22, February 2013.
 M.J. Lawler, K. Fujita, J. Lee, A.R. Schmidt, Y. Kohsaka, C.K. Kim, H. Eisaki,S. Uchida, J.C. Davis, J.P. Sethna, and E.A. Kim. Intra-unit-cell electronic nematicityof the high-TC copper-oxide pseudogap states. Nature (London), 466(7304):347–51,July 2010.
 P. Mallet, W. Sacks, D. Roditchev, D. Defourneau, and J. Klein. Spatial and energyvariation of the local density of states in the charge density wave phase of 2H-NbSe2.J. Vac. Sci. Technol. B, 14(2):1070, March 1996.
 Y.D. Chuang, A.D. Gromko, D.S. Dessau, T. Kimura, and Y. Tokura. Fermi surfacenesting and nanoscale fluctuating charge/orbital ordering in colossal magnetoresistiveoxides. Science, 292(5521):1509–13, May 2001.
 R. Liu, C. Olson, W. Tonjes, and R. Frindt. Momentum Dependent Spectral ChangesInduced by the Charge Density Wave in 2H-TaSe2 and the Implication on the CDWMechanism. Phys. Rev. Lett., 80(26):5762–5765, June 1998.
 J. van Wezel. Polar charge and orbital order in 2H-TaS2. Phys. Rev. B, 85(3):035131,January 2012.
 R. Barnett, A. Polkovnikov, E. Demler, W.G. Yin, and W. Ku. Coexistence of Gap-less Excitations and Commensurate Charge-Density Wave in the 2H Transition MetalDichalcogenides. Phys. Rev. Lett., 96(2):026406, January 2006.
 Y. Tokura. Orbital Physics in Transition-Metal Oxides. Science, 288(5465):462–468,April 2000.
 C.C. Lee, W.G. Yin, and W. Ku. Ferro-Orbital Order and Strong Magnetic Anisotropyin the Parent Compounds of Iron-Pnictide Superconductors. Phys. Rev. Lett.,103(26):267001–, December 2009.
 S. Nakatsuji, D. Hall, L. Balicas, Z. Fisk, K. Sugahara, M. Yoshioka, and Y. Maeno.Heavy-Mass Fermi Liquid near a Ferromagnetic Instability in Layered Ruthenates.Phys. Rev. Lett., 90(13):137202, April 2003.
 B.J. Kim, H. Jin, S.J. Moon, J.Y. Kim, B.G. Park, C.S. Leem, J. Yu, T.W. Noh,C. Kim, S.J. Oh, J.H. Park, V. Durairaj, G. Cao, and E. Rotenberg. Novel Jeff=1/2Mott State Induced by Relativistic Spin-Orbit Coupling in Sr2IrO4. Phys. Rev. Lett.,101(7):076402, August 2008.
 M.H. Whangbo and E. Canadell. Analogies between the concepts of molecular chem-istry and solid-state physics concerning structural instabilities. Electronic origin of thestructural modulations in layered transition metal dichalcogenides. J. Am. Chem. Soc.,114(24):9587–9600, November 1992.
 Y.Z. Ge and A. Liu. Effect of dimensionality and spin-orbit coupling on charge-density-wave transition in 2H-TaSe2. Phys. Rev. B, 86(10):104101, September 2012.
 B.C. Stipe, M.A. Rezaei, and W. Ho. Single-Molecule Vibrational Spectroscopy andMicroscopy. Science, 280(5370):1732–1735, June 1998.
 J. Nieminen, H. Lin, R. Markiewicz, and A. Bansil. Origin of the Electron-Hole Asym-metry in the Scanning Tunneling Spectrum of the High-Temperature Bi2Sr2CaCu2O8+δ
Superconductor. Phys. Rev. Lett., 102(3):037001, January 2009.
 N.F. Mott. The Basis of the Electron Theory of Metals, with Special Reference to theTransition Metals. Proc. Phys. Soc. London, Sec. A, 62(7):416–422, July 1949.
 P.A. Lee and X.G. Wen. Doping a Mott insulator: Physics of high-temperature super-conductivity. Reviews of Modern Physics, 78(1):17–85, January 2006.
 M. Tinkham. Group Theory and Quantum Mechanics. Courier Dover Publications,1964.
 M. Montalti, A. Credi, L. Prodi, and M. Teresa Gandolfi.Handbook of Photochemistry, Third Edition. CRC Press, 2006.
 M.K. Crawford, M.A. Subramanian, R.L. Harlow, J.A. Fernandez-Baca, Z.R. Wang,and D.C. Johnston. Structural and magnetic studies of Sr2IrO4. Phys. Rev. B,49(13):9198, April 1994.
 G. Cao, J. Bolivar, S. McCall, J.E. Crow, and R.P. Guertin. Weak ferromag-netism, metal-to-nonmetal transition, and negative differential resistivity in single-crystal Sr2IrO4. Phys. Rev. B, 57(18):R11039, May 1998.
 Y. Singh and P. Gegenwart. Antiferromagnetic Mott insulating state in single crystalsof the honeycomb lattice material Na2IrO3. Phys. Rev. B, 82(6):064412, August 2010.
 H. Okabe, M. Isobe, E. Takayama-Muromachi, A. Koda, S. Takeshita, M. Hiraishi,M. Miyazaki, R. Kadono, Y. Miyake, and J. Akimitsu. Ba2IrO4: A spin-orbit Mottinsulating quasi-two-dimensional antiferromagnet. Phys. Rev. B, 83(15):155118, April2011.
 J. Kim, D. Casa, M.H. Upton, T. Gog, Y.J. Kim, J.F. Mitchell, M. van Veenendaal,M. Daghofer, J. van den Brink, G. Khaliullin, and B.J. Kim. Magnetic ExcitationSpectra of Sr2IrO4 Probed by Resonant Inelastic X-Ray Scattering: Establishing Linksto Cuprate Superconductors. Phys. Rev. Lett., 108(17):177003, April 2012.
 F. Wang and T. Senthil. Twisted Hubbard Model for Sr2IrO4: Magnetism and PossibleHigh Temperature Superconductivity. Phys. Rev. Lett., 106(13):136402, March 2011.
 H. Watanabe, T. Shirakawa, and S. Yunoki. Microscopic Study of a Spin-Orbit-InducedMott Insulator in Ir Oxides. Phys. Rev. Lett., 105(21):216410, November 2010.
 A. Kitaev. Anyons in an exactly solved model and beyond. Annals of Physics, 321(1):2–111, January 2006.
 G. Jackeli and G. Khaliullin. Mott Insulators in the Strong Spin-Orbit CouplingLimit: From Heisenberg to a Quantum Compass and Kitaev Models. Phys. Rev. Lett.,102(1):017205, January 2009.
 H.C. Jiang, Z.C. Gu, X.L. Qi, and S. Trebst. Possible proximity of the Mott insulatingiridate Na2IrO3 to a topological phase: Phase diagram of the Heisenberg-Kitaev modelin a magnetic field. Phys. Rev. B, 83(24):245104, June 2011.
 R. Arita, J. Kunes, A.V. Kozhevnikov, A.G. Eguiluz, and M. Imada. Ab initio Studieson the Interplay between Spin-Orbit Interaction and Coulomb Correlation in Sr2IrO4
and Ba2IrO4. Phys. Rev. Lett., 108(8):086403, February 2012.
 D. Hsieh, F. Mahmood, D.H. Torchinsky, G. Cao, and N. Gedik. Observation of ametal-to-insulator transition with both Mott-Hubbard and Slater characteristics inSr2IrO4 from time-resolved photocarrier dynamics. Phys. Rev. B, 86(3):035128, July2012.
 T. Shimura, Y. Inaguma, T. Nakamura, M. Itoh, and Y. Morii. Structure and magneticproperties of Sr2−xAxIrO4 (A=Ca and Ba). Phys. Rev. B, 52(13):9143, October 1995.
 M. Ge, T.F. Qi, O.B. Korneta, D.E. DeLong, P. Schlottmann, W.P. Crummett, andG. Cao. Lattice-driven magnetoresistivity and metal-insulator transition in single-layered iridates. Phys. Rev. B, 84(10):100402, September 2011.
 H. Jin, H. Jeong, T. Ozaki, and J. Yu. Anisotropic exchange interactions of spin-orbit-integrated states in Sr2IrO4. Phys. Rev. B, 80(7):075112, August 2009.
 Q. Wang, Y. Cao, J.A. Waugh, S.R. Park, T.F. Qi, O.B. Korneta, G. Cao, andD.S. Dessau. Dimensionality controlled Mott transition and correlation effects in single-and bi-layer perovskite iridates. arXiv:1210.4141
 S.J. Moon, H. Jin, W.S. Choi, J.S. Lee, S.S.A. Seo, J. Yu, G. Cao, T.W. Noh, andY.S. Lee. Temperature dependence of the electronic structure of the Jeff = 1/2 Mottinsulator Sr2IrO4 studied by optical spectroscopy. Phys. Rev. B, 80(19):195110, Novem-ber 2009.
 R.M. Feenstra and P. Martensson. Fermi-Level Pinning at the Sb/GaAs(110) SurfaceStudied by Scanning Tunneling Spectroscopy. Phys. Rev. Lett., 61(4):447–450, July1988.
 C. Ye, P. Cai, R.Z. Yu, X.D. Zhou, W. Ruan, Q.Q. Liu, C.Q. Jin, and Y.Y. Wang.Visualizing the atomic-scale electronic structure of the Ca2CuO2Cl2 Mott insulator.Nat. Commun., 4:1365, January 2013.
 S. Moon, M. Kim, K. Kim, Y. Lee, J.Y. Kim, J.H. Park, B. Kim, S.J. Oh, S. Nakatsuji,Y. Maeno, I. Nagai, S. Ikeda, G. Cao, and T. Noh. Electronic structures of layeredperovskite Sr2MO4 (M=Ru, Rh, and Ir). Phys. Rev. B, 74(11):113104, September2006.
 C. Kittel. Introduction to Solid State Physics. John Wiley & Sons, 2004.
 B.H. Kim, G. Khaliullin, and B.I. Min. Magnetic Couplings, Optical Spectra, and Spin-Orbit Exciton in 5d Electron Mott Insulator Sr2IrO4. Phys. Rev. Lett., 109(16):167205,October 2012.
 H. Gretarsson, J.P. Clancy, X. Liu, J.P. Hill, E. Bozin, Y. Singh, S. Manni, P. Gegen-wart, J.H. Kim, A.H. Said, D. Casa, T. Gog, M.H. Upton, H.S. Kim, J. Yu,V.M. Katukuri, L. Hozoi, J. van den Brink, and Y.J. Kim. Crystal-Field Split-ting and Correlation Effect on the Electronic Structure of A2IrO3. Phys. Rev. Lett.,110(7):076402, February 2013.
 J. Dai. (unpublished).
 S. Uchida, T. Ido, H. Takagi, T. Arima, Y. Tokura, and S. Tajima. Optical spectra ofLa2−xSrxCuO4: Effect of carrier doping on the electronic structure of the CuO2 plane.Phys. Rev. B, 43(10):7942–7954, April 1991.
 Y.J. Kim, J.P. Hill, C.A. Burns, S. Wakimoto, R.J. Birgeneau, D. Casa, T. Gog, andC.T. Venkataraman. Resonant Inelastic X-Ray Scattering Study of Charge Excitationsin La2CuO4. Phys. Rev. Lett., 89(17):177003, October 2002.
 D.S. Ellis, J.P. Hill, S. Wakimoto, R.J. Birgeneau, D. Casa, T. Gog, and Y.J. Kim.Charge-transfer exciton in La2CuO4 probed with resonant inelastic x-ray scattering.Phys. Rev. B, 77(6):060501, February 2008.
 S. Fujiyama, H. Ohsumi, T. Komesu, J. Matsuno, B.J. Kim, M. Takata, T. Arima,and H. Takagi. Two-Dimensional Heisenberg Behavior of Jeff=1/2 Isospins in theParamagnetic State of the Spin-Orbital Mott Insulator Sr2IrO4. Phys. Rev. Lett.,108(24):247212, June 2012.
 S. Chikara, O. Korneta, W.P. Crummett, L.E. DeLong, P. Schlottmann, and G. Cao.Giant magnetoelectric effect in the Jeff=1/2 Mott insulator Sr2IrO4. Phys. Rev. B,80(14):140407, October 2009.
 R.S. Perry, F. Baumberger, L. Balicas, N. Kikugawa, N.J.C. Ingle, A. Rost, J.F. Mer-cure, Y. Maeno, Z.X. Shen, and A.P. Mackenzie. Sr2RhO4: a new, clean correlatedelectron metal. New J. Phys., 8(9):175, September 2006.
 F. Baumberger, N.J.C. Ingle, W. Meevasana, K.M. Shen, D.H. Lu, R.S. Perry,A.P. Mackenzie, Z. Hussain, D.J. Singh, and Z.X. Shen. Fermi Surface and Quasi-particle Excitations of Sr2RhO4. Phys. Rev. Lett., 96(24):246402, June 2006.
 R. Comin, G. Levy, B. Ludbrook, Z.H. Zhu, C.N. Veenstra, J.A. Rosen, Y. Singh,P. Gegenwart, D. Stricker, J.N. Hancock, D. van der Marel, I.S. Elfimov, and A. Dam-ascelli. Na2IrO3 as a Novel Relativistic Mott Insulator with a 340-meV Gap. Phys.Rev. Lett., 109(26):266406, December 2012.
 J. van den Brink, M.B.J. Meinders, J. Lorenzana, R. Eder, and G.A. Sawatzky. NewPhases in an Extended Hubbard Model Explicitly Including Atomic Polarizabilities.Phys. Rev. Lett., 75(25):4658–4661, December 1995.
 B. Bryant, Ch. Renner, Y. Tokunaga, Y. Tokura, and G. Aeppli. Imaging oxygendefects and their motion at a manganite surface. Nat. Commun., 2:212, January 2011.
 K.M. McElroy, J.H. Lee, J.A. Slezak, D.H. Lee, H. Eisaki, S. Uchida, andJ.C. Davis. Atomic-Scale Sources and Mechanism of Nanoscale Electronic Disorderin Bi2Sr2CaCu2O8+δ. Science, 309(5737):1048–52, August 2005.
 I. Zeljkovic, Z.J. Xu, J.S. Wen, G.D. Gu, R.S. Markiewicz, and J.E. Hoffman. Imagingthe impact of single oxygen atoms on superconducting Bi2+ySr2−yCaCu2O8+x. Science,337(6092):320–3, July 2012.
 O.B. Korneta, T.F. Qi, S. Chikara, S. Parkin, L.E. DeLong, P. Schlottmann, andG. Cao. Electron-doped Sr2IrO4−δ (0 < δ < 0.04): Evolution of a disordered Jeff = 1/2Mott insulator into an exotic metallic state. Phys. Rev. B, 82(11):115117, September2010.
 T.F. Qi, O.B. Korneta, S. Chikara, M. Ge, S. Parkin, L.E. De Long, P. Schlottmann,and G. Cao. Electron doped Sr2IrO4−δ (0 < δ < 0.04): Evolution of a disordered Jeff =1/2 Mott insulator into an exotic metallic state. J. App. Phys., 109(7):07D906, March2011.